A
PARADIGM CALLED
MAGNETISM
This page intentionally left blank
A
PARADIGM CALLED
MAGNETISM
Sushanta Dattagupta...

Author:
Sushanta Dattagupta

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

A

PARADIGM CALLED

MAGNETISM

This page intentionally left blank

A

PARADIGM CALLED

MAGNETISM

Sushanta Dattagupta Indian Institute of Science Education & Research Kolkata, India

World Scientific NEW JERSEY . LONDON . SINGAPORE . BEIJING . SHANGHAI . HONG KONG . TAIPEI . CHENNAI

A-PDF Merger DEMO : Purchase from www.A-PDF.com to remove the watermark

Published by World Scientific Publishing Co. Pte. Ltd. 5 Toh Tuck Link, Singapore 596224 USA office: 27 Warren Street, Suite 401-402, Hackensack, NJ 07601 UK office: 57 Shelton Street, Covent Garden, London WC2H 9HE

British Library Cataloguing-in-Publication Data A catalogue record for this book is available from the British Library.

Images on cover design are from http://www.indiaart.com/Online_Exhibitions/online_exhibitions_1.html

A PARADIGM CALLED MAGNETISM Copyright © 2008 by World Scientific Publishing Co. Pte. Ltd. All rights reserved. This book, or parts thereof, may not be reproduced in any form or by any means, electronic or mechanical, including photocopying, recording or any information storage and retrieval system now known or to be invented, without written permission from the Publisher.

For photocopying of material in this volume, please pay a copying fee through the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, USA. In this case permission to photocopy is not required from the publisher.

ISBN-13 978-981-281-386-2 ISBN-10 981-281-386-1

Printed in Singapore.

Benjamin - A Paradigm Called Magnetism.pmd 1

9/2/2008, 5:40 PM

To the cause of integrated Science Education and Research, in India.

This page intentionally left blank

Preface

Magnetism is truly a very old subject. The first reference to a magnetic material, magnetite or the famed loadstone, can be found in Greek literature in astonishingly early times like 800 B.C. Yet the subject remains modern. It appeals to extremely basic issues of physics– magnetism as a material property is a direct result of one of the fundamental forces of nature governed by electromagnetic interactions. At the same time, this property forms the core of technology, influencing power-generation, biomedical applications through, for instance, magnetic resonance imaging, computer industry with the aid of memory devices and chips, just to name a few. Our objective in this volume is not to dwell on the myriad applications of Magnetism but to highlight the rich structure of its theory. It is remarkable to recount how many extraordinary ideas of physics ensue while teaching a course in Magnetism. To mention some: the first instance of velocity-dependent potentials in Mechanics is encountered in treating the Lorentz force on a charged particle in a magnetic field, the first example of the violation of time reversal is stumbled upon when we consider the Zeeman interaction of a spin in an external magnetic field, and so on. Given this background to the wide applicability of the concepts of Magnetism, the purpose of these Lecture Notes is to further amplify how the subject has influenced developments in other diverse areas of Physics and how models used in Magnetism can help to clarify a variety of apparently unrelated phenomena. Magnetism is essentially a quantum mechanical subject. Yet its classical limits such as those described by Heisenberg or Ising-like models have far reaching applications to a

vii

viii

Preface

plethora of topics in phase transitions. Thus, while the ideas of symmetry-breaking and scaling first appeared in Magnetism, they soon pervaded other topics of not just condensed matter physics, but even distant terrains of field theory and high energy physics. Similarly, the concepts of disorder and frustration, embedded in magnetic spin glass systems, are also common to structural glasses. In the domain of nonequilibrium effects too, examples derived from Magnetism help to elucidate the underlying issues of relaxation and dissipation. With the preceding preamble, the Lecture notes are chapter-wise divided as follows. Chapter 1, consisting of three sections, deals with the by-now well-known phenomena which first appeared in the context of Magnetism but have had important bearing in many other subjects. In section 1.1, we discuss the Mermin-Wagner-Berezinskii theorem on symmetry-breaking in the context of the Heisenberg magnet and its implications in φ 4 field theory. The latter forms the backbone of section 1.2 that is devoted to universality and consequent scaling relations which are the underlying concepts in critical point phenomena. In section 1.3 we discuss the issue of multicriticality and point out how the models originally introduced to describe this phenomenon in what are called metamagnets, found their application to tricritical points in 3He - 4He mixtures and even to bicriticality and tetracriticality in an open, nonequilibrium system such as a two-mode ring laser. From chapter 2 onwards, we turn to more recent topics. In chapter 2, we introduce the contemporarily relevant topic of the quantum critical point, again in the context of the Ising model but now in a transverse magnetic field, which finds its realization in rare-earth magnetism. The model helps illustrate the occurrence of quantum phase transitions in a variety of phenomena. The same model allows us to deal with the inter-connected concept of disorder and frustration, which is the subject of chapter 3. Again, the important ideas were first observed in dilute magnets alloyed with metals, called spin glasses. In chapter 4, we move from equilibrium to nonequilibrium statistical mechanics and show how the well-established ideas of spin-lattice and spin-spin relaxations, which are at the heart of magnetic resonance systems, can be further developed to obtain coarse-grained models of phase ordering and pattern formation, seen in many systems as competition between nonlinear interactions and

Preface

ix

nonequilibrium effects. In chapter 5, we discuss important nonequilibrium phenomena seen in an assembly of single-domain nanomagnetic particles. The concomitant relaxation and memory effects are found to be a consequence of the interplay between polydispersity and inter-particle interactions. Similar memory or aging effects are observed in very different systems of relaxor ferroelectrics, shapememory ferroelectric materials and structural glasses. The concepts discussed in chapter 4 in the context of magnetic response and relaxation behaviour find their counterparts in the recently-developed subject of dissipative quantum systems, discussed in detail in chapter 6. Therein we analyze the significance of coherence to decoherence transitions using a magnetic paradigm of Diamagnetism, which is intrinsically a quantum phenomenon, for which the boundary of the container plays a critical role. Thus dissipative diamagnetism is prototypical of decoherence in mesoscopic structures. Our final example is from a large spin quantum system that finds its realization in molecular magnets, and in which mesoscopic quantum tunneling can be seen. The influence of environment-induced dissipation makes this system yet another example of observing coherence to decoherence in quantum to classical crossover phenomena. Acknowledgments I would like to thank the Department of Science and Technology, New Delhi for awarding me the J.C. Bose Fellowship, which enabled me to complete this project. The staff at World Scientific Press in Singapore deserve special praise for being so patient with me despite me missing so many deadlines for manuscript submission. My wife Ranu, daughters Shahana and Sharmishtha, and numerous colleague island friends have been strongly supportive during my challenging days of transition, when this manuscript was being written. I record my warmest gratitude to them. Finally, I thank Manas Roy for help with the figures and Immanuel Alexander for efficient word-processing. Sushanta Dattagupta

This page intentionally left blank

Contents

Preface

vii

1. An Assortment of Well-Established Concepts 1 1.1 Symmetry-Breaking ................................................................................ 1 1.2 Critical Phenomena and Scaling ............................................................. 9 1.3 Multicriticality ...................................................................................... 16 1.4 Multicriticality in an Open System of Two-Mode Lasers .................... 24 2. Quantum Phase Transition: Transverse Ising Model and Other Systems 2.1 Introductory Remarks ........................................................................... 2.2 The Mean Field Theory of TIM ............................................................ 2.3 The Quantum Magnet LiHoF4 .............................................................. 2.4 Quantum Statistical Mechanics ............................................................

29 29 32 36 41

3. Glass Transitions 3.1 Preamble – Magnetic Glass, Quantum Glass, Spin Glass, Proton Glass and Structural Glass ........................................................ 3.2 Magnetic Glass: Li Hox Y1-xF4 ............................................................ 3.3 Quantum Glass: Li Hox Y1-xF4 in a Transverse Field ........................... 3.4 Spin Glasses .......................................................................................... 3.5 Proton Glasses ...................................................................................... 3.6 Structural Glasses .................................................................................

47 47 48 57 59 62 64

4. Relaxation Effects 4.1 Introductory Remarks ........................................................................... 4.2 Single Spin Kinetics in Equilibrium ..................................................... 4.3 Non-Equilibrium Response of a Single Spin ........................................ 4.4 Effects of Interaction on Relaxation .....................................................

69 69 71 78 83

xi

xii

Contents

5. Memory in Nanomagnets 95 5.1 Introduction to the Physics of Single Domain Nanomagnetic Particles ................................................................................................ 95 5.2 Rotational Brownian Motion, the Kramers Problems and Susceptibility ...................................................................................... 106 5.3 Experiments: Stern-Gerlach and Mössbauer Spectroscopy ................ 117 6. Dissipative Quantum Systems 6.1 Introduction ........................................................................................ 6.2 Nonequilibrium Statistical Mechanics ................................................ 6.3 Spin-Boson Hamiltonian .................................................................... 6.4 Dissipative Diamagnetism .................................................................. 6.5 Spin Tunneling and Coherence-Decoherence Phenomenon ...............

139 139 142 148 157 169

References

179

Index

189

Chapter 1

An Assortment of Well-Established Concepts

1.1. Symmetry-Breaking The dynamics of a many body system are determined in terms of a Hamiltonian. The Hamiltonian is characterized by its invariance properties under all transformations that belong to a group, reflecting the underlying symmetries of the system. An extremely rich example of such a system is the one governed by interacting magnetic spins S and described by what is called the Heinsenberg Hamiltonian: H =− J Si ⋅ Sj . (1.1)

∑

The summation is over sites i and j, and is restricted to nearest neighbours, as indicated by the angular brackets < >. The term J is usually referred to as the exchange interaction [1-5]. We may now enlist all the invariance properties of H . The most basic of all these, as is indeed the fundamental attribute of all mechanical systems, is the invariance under time translation. The implication of this invariance is that the total energy is constant, as it must be for a conservative mechanical system. The second invariance property, again shared by most mechanical systems, is the one exhibited under time reversal. As the time t is reversed to −t, each spin operator such as Si has its sign flipped, because S transforms like the orbital angular momentum operator. There is however no overall change in sign for the pair i and j. Time reversal symmetry is fundamental to electromagnetic forces and is broken only due to dissipation, or the presence of an external magnetic field. The third property, which is what we would like to focus onto, 1

2

A Paradigm Called Magnetism

relates to the invariance of H under the simultaneous rotations of all spins through an arbitrary angle about an arbitrary axis. The group of transformations that leaves the Hamiltonian invariant is the symmetry group, denoted by G. If the Heisenberg Hamiltonian does not make a distinction between different orientations, as discussed above, how does it then describe ferromagnetism which is associated with a unique directionality of the magnetization? Recall that the thermodynamic state of a system is governed by the minimum of the Helmholtz free energy F = U – TS, U being the internal energy, S the entropy and T the temperature. For instance, for the magnetic system at hand, the system would choose those spin configurations for which F is minimized. Thus, at high temperatures, the entropy dominates and the maximally disordered state has the highest entropy. This implies that the high temperature equilibrium state is paramagnetic with no average alignment of spin, i.e. the magnetization is zero. Therefore, the paramagnetic phase is invariant under the same group G as its Hamiltonian. On the other hand, at low temperatures, U dominates over TS and the ground state of H is the one in which all the spins are aligned along the same direction. (Note the negative sign in the right hand side of Eq. (1).) This low temperature equilibrium phase is a ferromagnetic one with nonzero average spin <S> = <Si >, independent of the site index i, or equivalently a magnetization, m = µVo–1 <S>, Vo being the volume of a unit cell and µ the magnetic moment per spin. At a critical temperature Tc called the Curie temperature the system undergoes a phase transition from the entropy dominated paramagnetic state to the energy dominated ferromagnetic state. Thus the magnetization m, which is zero in the paramagnetic phase and becomes non-zero in the ferromagnetic phase, is appropriately called the order parameter of the low temperature phase. It is invariant under rotations about an axis parallel to itself but changes under rotations about all axes that are oblique to itself. Therefore, the ordered phase has a lower symmetry than the full symmetry of the group G — it is a broken symmetry phase, as it breaks the symmetry of the Hamiltonian [6, 7]. The important concept of symmetry-breaking transitions, as enumerated above, transcends the subject of Magnetism to many

An Assortment of Well-Established Concepts

3

other areas of Condensed Matter Physics and even to Quantum Field Theory and Particle Physics [8]. Indeed many of the ideas of symmetry and symmetry-breaking transitions in Magnetism, as encapsulated in the Heisenberg or Heisenberg-like models, can be carried over to different fields. We may recall that the most common form of phase transitions in condensed matter physics is encountered in the case of fluids (gases or liquids). A fluid is the highest symmetry phase of matter which is invariant under the Euclidean group of all translations, rotations and reflections. As the external field such as pressure and temperature are varied one sees a series of phase transitions. The most common low temperature phase is a crystalline solid for which the symmetry is lowered from that of the fluid phase. As it turns out the gas-liquid phase transition can be discussed in complete analogy with the magnetic phase transition. While this will be dealt with in Sec. 2 below we want to mention here that in Quantum Field Theory, the idea of symmetrybreaking in a Heisenberg magnet finds its echo in the Lagrangian of n-coupled scalar fields in what is called a φ 4 theory. Although the Lagrangian and hence the equations of motion are invariant under a continuous group of transformations, the ground state, called now the vacuum, is not invariant — the symmetry appears spontaneously broken. This phenomenon is completely akin to a Heisenberg magnet which exhibits spontaneous (i.e. in the absence of an applied magnetic field) magnetization below the Curie temperature. Further, just as in the case of Heisenberg magnets wherein low temperature excitations are described by spin waves (whose quanta are magnons), the consequence of continuous symmetry-breaking in field theory is the appearance of massless excitations called the Goldstone Bosons. Indeed, it is this similarity between Magnetism and Particle Physics which has helped establish the deep relationship between Field Theory and Statistical Mechanics [9-11]. To further underscore this similarity, mentioned in the paragraph above, we may recall the famous Mermin-Wagner-Berezinskii (MWB) theorem [12-14]. It states that a system with a continuous symmetry (such as the Heisenberg model under continuous rotations) cannot have a spontaneously broken symmetry in dimensions less than or equal to two. The theorem is most conveniently proved in a simpler version of the

4

A Paradigm Called Magnetism

Heisenberg model called the XY-model. In the XY-model the longitudinal components (along the Ƶ-axis about which the symmetry of the Heisenberg model is expected to be broken) are assumed suppressed. Thus Eq. (1.1) yields

Hxy = − J

∑ (S S

ix jx

+ Siy Sjy ).

(1.2)

The Hamiltonian in Eq. (2), like the one in Eq. (1.1), is invariant under continuous and arbitrary rotations about the ƶ-axis. In the classical limit Eq. (1.2) may be written as Hxy =− J

∑ cos(θ − θ ) . i

j

(1.3)

Further, in order to obtain the continuous limit of Eq. (1.3) in which the lattice spacing a is arbitrarily small, we can expand the cosine term to yield H=

J 4

∑ γ (θ ij

i

− θj )2 − ξ JN + higher order terms .

(1.4)

ij

In Eq. (1.4), is the number of nearest neighbours (the ‘coordination number’ of the lattice). The restriction on the summations over i and j being over nearest neighbours (indicated by angular brackets in Eq. (1.3)) is removed but is reimposed through the introduction of a matrix γij which is defined as

γij = 1, if i and j are nearest neighbors , = O, otherwise.

(1.5)

Neglecting the constant and the higher order terms in Eq. (1.4) the continuum version is

Hxy =

1 d d xp[∇θ ( x )]2 , 2

∫

where d is the spatial dimensionality and

(1.6)

An Assortment of Well-Established Concepts

p=

ξJ 2d

a2− d .

5

(1.7)

In the XY model the spin vector can point in any direction in the XY-plane, but if the symmetry is broken, one direction is preferred. Assuming that direction to be the X-axis the order parameter is 1 cos Dθe e . Z

1.8

where Z is the partition function and β = (kBT)–1, kB being the Boltzmann constant and T the temperature. Using the ‘Gaussian’ property of Hxy due to which all cumulants of the fluctuations in θ (x) beyond the second order vanish, we find 1

− < cos θ ( x ) > = e 2 .

(1.9)

Furthermore

< θ 2 (x) > = −

∑ q

∂ 1 ∂ βρ q 2 2

ln Z q ,

(1.10)

where # is the wave vector that is Fourier-conjugate to , and 1

2π 2 Zq = βρ q 2

(1.11)

Thus < θ 2 (x) > =

1

∑ βρ q q

2

.

(1.12)

which, in the continuum limit yields 1 ddq 1 1 Λd − 2 < θ 2( x ) > = = , 2βρ (2π ) d q 2 4π 2 ρβ (d − 2)

(1.13)

where Λ is the wave number cut off. Equation (1.13) measures the degree to which the order parameter value is diminished from its zero

6

A Paradigm Called Magnetism

temperature (saturation) value due to classical thermal fluctuations. Evidently as the dimension d approaches the value 2 the fluctuations grow inordinately thereby destroying the order (cf. Eq. (1.9)). This result then proves the celebrated MWB theorem by establishing that fluctuations destroy long range order for a system with continuous symmetry in dimensions less than or equal to two. Physically speaking, the long-wavelength (low q) modes make ‘weighty’ contributions in low dimensions, thermal excitation of which averages out the orientation of the average spin angular momentum. The MWB theorem, first derived in the context of magnetism, has been restated by Coleman in Field Theory. As mentioned earlier, spontaneous symmetry-breaking yields a zero mass Goldstone boson. However, in a two-dimensional space-time it is not possible to construct a massless scalar field operator due to severe infrared (or large wavelength) divergences, as indicated above [15]. While the XY-model discussed above is one kind of anisotropy-limit of the Heisenberg model, a different kind of anisotropy ensues when the transverse components of the spin are suppressed and only the longitudinal components are led to interact. This yields the much studied Ising model the Hamiltonian of which can be written as [16, 17] HIS =− J

∑S S

iz jz

.

(1.14)

Unlike the Heisenberg or the XY-model, the Ising model is evidently endowed with discrete symmetry. This symmetry is classified under a group called Z2 that comprises just two elements: the identity and an element whose square is the identity. This Ising or Z2 symmetry is broken in those phase transitions which have just two ordered states with order parameters simply differing in sign. Naturally there is no MWB theorem in the Ising case, which does exhibit a phase transition in two dimensions. The discrete symmetry has a further consequence that there is no mass-less Goldstone bosons — the spin wave spectrum (depicting the magnon frequency versus the wave number) has a gap at large wavelengths [18].

An Assortment of Well-Established Concepts

7

The Ising model has a special place in history as it provides a vindication of the subject of statistical mechanics through the path breaking work of Onsager who obtained an exact solution for the partition function of the model in two dimensions. Thus the existence of phase transition, a phenomenon that occupies the centre stage in the subject of thermodynamics, could be demonstrated in terms of a microscopic theory namely that of statistical physics [19]. It is interesting to note that although the Ising model was first introduced as a model of a Heisenberg-like magnet in the limit of extreme anisotropy, such as due to crystal field effects, the majority of its applications is in different fields such as gas-liquid transitions or ordering in alloys. Thus, in the context of gas-liquid transitions, it is a common practice to think of a lattice-gas model wherein a lattice is imagined to consist of cells. Each cell can be occupied by a liquid-like particle, or be empty, to depict a gas-like particle. Hence, the basic statistical variable is a binary one, like in the Ising magnet, but now is a ‘pseudo spin’ whose upward projection indicates an occupied cell whereas a downward projection implies a vacant cell. If we define the order parameter as the deviation of the density from its average (of the liquid and gas densities of the corresponding coexisting phases) value, the ordered states of liquid and gas are again characterized by equal and opposite (in sign) order parameters, exactly as in the case of the Ising magnet. Indeed this identification of the order parameter allows us to describe the phenomena near the critical point of a gas-liquid phase transition in complete analogy with a paramagnet-to-ferromagnet transition [17]. This is further linked with the concept of ‘universality’, a subject of Sec. 1.2. As mentioned above, the discrete binary symmetry of the Ising model finds yet another application to materials science. Consider then a solid alloy of just two elements. Each lattice site is imagined to be occupied by either an A or a B-type of atom. Thus the occupation variable is once again an Ising pseudo-spin, but now one encounters two distinct phenomena depending on whether the exchange parameter J in Eq. (1.14) is positive or negative. If J > 0, corresponding to ferromagnetic ordering of the spins in the low-temperature phase, one would see clustering of A-rich (i.e. domains of up spins) and B-rich

8

A Paradigm Called Magnetism

(i.e. domains of down-spins) phases. The order parameter now is naturally a composition variable, depicting the fractional concentration of one or the other (A or B) type of atoms. Although this analogy between what is called the phase ordering of alloys and the Ising ferromagnet is complete as far as static thermal properties are concerned, the kinetics in the two cases are quite different. If one imagines to ‘quench’ (i.e. rapidly cool) a spin disordered paramagnet below its Curie temperature, kinetics of ferromagnetic ordering proceed via preferential flipping of spins from one projection to the other. Thus the order parameter, or the magnetization in the present case, is not conserved. On the other hand, in the alloy case, quenching from the disordered (or paramagnetic-like) phase in which the A and B atoms are randomly distributed, to the ordered phase does not imply transmutation of the chemical identify of atoms but simply an interchange of A and B atoms over neighbouring lattice sites. Therefore, the order parameter is now conserved. This difference between conserved and non-conserved order parameter kinetics leads to distinct morphology of domain growth in the two cases [20]. We now discuss the opposite J < 0 (antiferromagnetic) case. It is clear from Eq. (1.14) that alternate up and down orientations of the spins lower the energy. Correspondingly, the alloy case leads to alternate ordering of the A and B atoms, reflecting the fact that unlike atoms like each other in contrast to the phase-ordering case wherein like atoms prefer to agglomerate together. The J < 0 phase transition is appropriately referred to as the order-disorder transition as can be seen, for example, in beta-brass: a 50-50 admixture of copper and zinc on a BCC lattice. At high temperatures, the Cu and Zn atoms occupy two sub-lattices A and B with equal probability. In the low temperature ordered phase, one set of atoms segregates into the sub-lattice A while the other segregates into the other sub-lattice B. The order parameter: C = CCu,A – CCu,B, where C = CCu,A(CCu,B) is the concentration of Cu atoms in the sub-lattice A(B), is the exact analog of the so-called staggered magnetization of an antiferromagnet. What about kinetics? It is important to note that although kinetic processes involving mutual exchange of A and B atoms on neighbouring sub-lattices conserves the

An Assortment of Well-Established Concepts

9

number of A and B atoms, they do not conserve the sub-lattice order parameter. From the above discussion, it is apparent that a whole range of solidification and ordering phenomena in materials science has derived rich dividends from the analysis of the Ising model in magnetism. In addition to the example of alloys, other transformations that have Ising symmetry are ferroelectric and ferroelastic transitions in which the order parameter is an electric polarization or a spontaneously developed strain, respectively [21]. Further generalization of the Z2 Ising symmetry to Zn symmetry yields yet other interesting phenomena of discrete symmetry changes in condensed matter physics. Thus, the n = 3 case known as the Potts model [22], leads to surface ordering such as krypton absorbed on graphite in which one finds three equivalent ground states commensurate with one Kr atom for every three unit cells of the graphite lattice [23]. We now have a Z3 symmetry-broken transition from a fluid to the commensurate state.

1.2. Critical Phenomena and Scaling Our stated objective in these Lecture Notes has been to employ models and phenomena in Magnetism in order to elucidate developments of similar ideas in other fields. To this end we discuss in this section the extremely important topic of critical phenomena and scaling [24]. Indeed it is not an exaggeration to state that the most profound theoretical advance in physics in the last quarter of the last century has been the successful application of the Renormalization Group (RG) to the critical point phenomena, exploiting and using the ideas of scaling [25-27]. Again it is the second order paramagnetic to ferromagnetic transition at the critical (Curie) point that formed the standard paradigm of critical phenomena, and the Ising and similar models of magnetism became the happy hunting ground for applying RG ideas. We first discuss phase diagrams indicating first order transitions across a twophase co-existing line culminating at an isolated point of second order transition, called the critical point, and then introduce the idea of scaling.

10

A Paradigm Called Magnetism

Fig. 1.1. The magnetic field H, applied in the laboratory along the Ising easy axis, is plotted versus the temperature T. The critical point, indicated by a dot, occurs at H = 0 and T = Tc .

While drawing phase diagrams we follow the Griffiths nomenclature of thermodynamic ‘field’ variables such as temperature, pressure, magnetic field intensity, etc., which remain the same for co-existing phases, and ‘density’ variables such as number density, composition, specific volume, magnetization, etc., which acquire distinct values across the co-existence line [28]. The phase diagrams are drawn in either pure field variables space or mixed field-density variables space. An example of the former for a magnet is shown in Fig. 1.1, in which the magnetic field H is plotted versus the temperature T for an Ising model. The coexistence line (for H = 0) is shown as a solid line for T < Tc and a dashed line for T > Tc ; the black dot is the critical point. Recall from Sec. 1.1 that the symmetry-breaking transition in a magnet occurs spontaneously i.e., in the absence of an external magnetic field. Thus the H = 0 line in Fig. 1.1 plays a special role as it is indeed the co-existence line. Thus, experimentally if one had simply gone on to reduce the temperature one would naturally approach Tc from above along the dashed line. Recalling the Z2 discrete symmetry of a Ising Model (cf. Sec. 1.1) the paramagnetic phase above Tc is a spindisordered phase for which the macroscopic magnetization M is zero, because it is equally likely to find a spin pointing up or down. The

An Assortment of Well-Established Concepts

11

situation is illustrated in Fig. 1.2 which shows the thermodynamic Free Energy F versus M. The curve is schematically a parabola, near M = 0 and the thermodynamically stable state for which F is minimum corresponds to M = 0. As T approaches and becomes very near to Tc the curvature of F near M = 0 becomes vanishingly small (Fig. 1.3) until T is decreased just below Tc when F acquires a double-well structure (Fig. 1.4).

Fig. 1.2. A schematic sketch of the Free Energy F versus the magnetization M, for T Tc .

The two minima of F in Fig. 1.4 are degenerate (i.e. they have the same value of F) corresponding to macroscopic regions in each of which the spins point up or down — the Z2 symmetry is spontaneously broken. The corresponding situation is illustrated in Fig. 1.5 which depictsthe phase diagram in the mixed density-field variables space, i.e., M versus T. The two minima of F in Fig. 1.4 are denoted by M+ and M– (M– = −M+) which are to be read off from the two ends of what is called a tie line, indicated by a solid vertical line in Fig. 1.5. The length of the tie line goes on increasing as the temperature T goes on decreasing until at T = 0 M acquires the saturation value Ms. The entire phenomena, described above, are visualized to occur on the two phase co-existence line (i.e. the solid line in Fig. 1.1). Thus a point on the co-existence line in the pure field space (i.e. in Fig. 1.1), for T < Tc fans out into a line in the mixed space of Fig. 1.5, a feature that is generic and is in conformity with the Gibbs Phase Rule [29].

12

A Paradigm Called Magnetism

Fig. 1.3. A schematic sketch of the Free Energy F versus the magnetization M, for T → Tc .

Fig. 1.4. A schematic sketch of the Free Energy F versus the magnetization M, for T just below Tc .

Having discussed the magnetic phase diagram we now analyse in parallel the phase diagram of a fluid that exhibits a gas-liquid phase transition. Recall from Sec. 1.1 that the gas-liquid transition can be described in terms of a lattice gas model which is directly derived from the Ising model. Thus it is not surprising that the two sets of phase diagrams have striking similarties, as well as important dissimilarities. The field that plays the role of the magnetic intensity in a fluid is the

An Assortment of Well-Established Concepts

13

pressure P and the conjugate variable, analogous to the magnetization M, is the specific volume V. The P-T phase diagram for a fluid, in the pure field variable space and akin to Fig. 1.1, is shown in Fig. 1.6. Again the solid line (but now a curved one) is a two-phase co-existence line on which the gas and the liquid phases co-exist with the same (degenerate) value of the Free Energy (cf., Fig. 1.4). Further, like in the magnet case, one can go continuously around the critical point (Pc, Tc) from the gas phase to the liquid phase and vice-versa. However, for a fluid, we are more accustomed to think in terms of a first order transition in which the specific volume V jumps discontinuously as we cross the co-existence line, accompanied by a latent heat of vaporization unlike in Fig. 1.5 in which the magnetization grows continuously from its value as T is decreased below Tc. This difference between the two cases is amplified below:

Fig. 1.5 The co-existence line (parabola-shaped) depicting the magnetization M versus the temperature T. The vertical lines are tie-lines, defining the values of M for co-existing phases.

In the magnet case the co-existence line corresponds to H = 0, as discussed earlier. This relates to the fundamental symmetry of time reversal invariance, discussed in Sec. 1, which implies that for H = 0 the up and down spin projections are equivalent. There is no such symmetry in the fluid case, hence Pc is non-zero and crossing the two-phase co-existence line (the solid one in Fig. 1.6) along an isobar (i.e. constant pressure) or along an isotherm (i.e. constant temperature) would lead to a discontinuous jump of the specific volume.

14

A Paradigm Called Magnetism

Fig. 1.6. The pressure P versus temperature T for a fluid. The solid line is the gas-liquid co-existence line, the continuation of which (the dashed line) is the critical isochore.

How can then one establish a similarity between the magnet and the fluid cases? The clue is to find the right ‘path’ of approach to the critical point. That particular path turns out to be the critical isochore (the dashed line in Fig. 1.6) along which the density is fixed at its critical value, say nc. Defining then the order parameter of the gas-liquid transition as φ = n – nc, φ remains zero along the dashed line, exactly as in Fig. 1.1 for the magnet case, until one reaches below the ‘critical point’ (Pc, Tc) where from φ grows continuously. The critical point, an isolated point of a second order phase transition as discussed above, is a very special point in the phase diagram of a system. The special nature of the point is related to the fact that certain thermodynamic response functions show divergent behaviour as a function of t = (T – Tc)/Tc, as the temperature T approaches the critical temperature Tc from above. Again, the most widely studied response function turns out to be the one relevant for magnetism and that is the magnetic susceptibility $, which measures the linear response of the magnetization to an applied magnetic field. The function χ diverges as t –γ, as t → 0+ where γ is referred to as a critical exponent. What is further remarkable is not only that a very different property, namely the isothermal compressibility for a different system, i.e. a fluid, is characterized by the same divergent behaviour but that the value of γ is

An Assortment of Well-Established Concepts

15

identical to that of an Ising magnet. This follows from the mapping of the Ising model to a lattice-gas model, as mentioned above. The result is quite astonishing because the two systems under consideration are governed by very different interactions and very distinct physical properties. Indeed it is not just a fluid that shows this commonality of behaviour of its response function near the critical point with a magnet but so do other different physical systems e.g. a ferroelectric or an order-disorder alloy, all of which are said to belong to the so-called Ising universality class. This brings us to the issue of universality which links a whole lot of physically different systems based on the common factors of spatial dimensionality d, the dimension n of the order parameter (=1 for the Ising case) and the range of interactions. The astounding statement of universality is that critical exponents like γ (or β which measures how the order parameter such as the magnetization vanishes continuously as T → Tc) are universal. Thus, to the extent that critical phenomena at a gas-liquid transition in a fluid and a paramagnetferromagnet transition in a magnet are describable in terms of the same Ising model (with Z2 symmetry and short-ranged interactions) in three dimensions, the two very different systems are characterized by the same critical exponents [30]. The universality follows from a very general thermodynamic principle that potentials such as the free energy, are generalized homogeneous functions of temperature and other fields in the vicinity of the critical point. The homogeneity leads to certain scale invariance, the essential idea of which can be summarized as follows. The occurrence of a critical point is in some sense the culmination of the battle between the energy, which dictates order and the entropy, which embodies disorder. Thus, fluctuations, measured by the correlation function of spins at different sites of an Ising magnet, for instance, grow inordinately. Concomitantly the correlation length, that characterizes the distance over which a pair of spins is correlated, diverges at Tc. Thus all other length scales become irrelevant and the only length scale that matters near Tc is the correlation length. This then is the notion of scaling which allows us to estimate how thermodynamic functions and correlations vary with temperature from the dependence of the correlation length on temperature.

16

A Paradigm Called Magnetism

It is this twin concept of universality and scaling that led to the successful application of the renormalization group (RG) by Wilson and others to the critical point phenomena [31]. The RG provides a computational scheme for a class of problems for which fluctuations at multitudes of length scales become important. This scheme was successfully applied by Wilson in the early 1970s to the calculation of critical exponents that led to the theoretical validation of universality. Wilson’s original calculation was in the context of field theories in which one introduces a local order parameter, treated as a continuous classical field and the partition function is written as an integral over all possible values of the local order parameter at all space points. But, the most illuminating treatment of RG theory dates back to 1966 when Kadanoff provided a heuristic explanation of scaling, again in the context of an Ising magnet. This real space treatment called Kadanoff construction, does in fact yield a platform on which to build Wilson’s RG which allows for explicit calculations of critical exponents and scaling relations. The Kadanoff construction can be exactly carried out for the one-dimensional Isuing model and leads to higher dimensional generalization following an approximate method called the Migdal (1975)- Kadanoff (1976) procedure [32]. A natural extension of the procedure, first developed for an Ising model in 1 + ε dimensions, can be nicely extended to the problem of Krypton adsorbed on graphite which, as mentioned at the end of Chapter 1.1, can be described by the Potts model of Z3 symmetry [22].

1.3. Multicriticality The phase diagram for an Ising magnet, discussed in Sec. 1.2 (cf. Fig. 1.1), consists of a single line (for H = 0) along the T-axis. The temperature T is thus the only disordering field. Increase in T causes a first order line of two-phase co-existence to terminate at a point called the critical point which is an isolated point of second order transition. What happens when there is more than one disordering field? In the sense of the Gibbs Phase Rule we will have more “degrees of freedom”, in which case, is it possible that we will have a line of critical points in a

An Assortment of Well-Established Concepts

17

higher dimensional phase diagram? Can we generate special critical points which can be reached by simultaneously fixing two or more disordering fields? The answer is YES, and such critical points, called multi-critical points are the subject of this section. The present analysis is based on what is now called the Blume-Capel model [33, 34]. Imagine a Hamiltonian which describes an Ising-type interaction between nearest neighbours which however are now spin-1 ions in a lattice that are subject also to a crystal field ∆:

H=−J

∑S S

ij jz

+∆

2 iz ,

∑S

∆>0

(1.15)

i

Clearly, the crystal field terms would simply be a constant for the ordinary spin half Ising model discussed hitherto. Here Si = ±1 or 0 and one now can consider two disordering fields T and ∆ shown in Fig. 1.7 For ∆ = 0, we are back to our earlier Ising case, in which we have the usual ferromagnetic to paramagnetic transition but now occurring along the ordinate (in constrast to Fig. 1.1). For small enough ∆ the single ion energy levels Si = ±1 lie not much higher than Si = 0 singlet and so the exchange interaction remains operative. Under this condition, mean field calculations suggest that the paramagnetic-ferromagnetic transition continues to be of second order as in the ordinary Ising model. As ∆ is increased one sees a line of critical points (the solid line in Fig. 1.7), until beyond a critical value ∆c, the transition changes into a first order one and the cross-over occurs at what is called a tricritical point [35]. As ∆ is increased still further, the transition temperature decreases and goes to zero. This is so because, for a large value of ∆ the Si = ±1 levels become inaccessible and hence the exchange interaction becomes inoperative. The following features about the various terms in the Hamiltonian in Eq. (1.15) are worth noting in our understanding of tri-critical behaviour. First, one has the usual magnetic order M = <Si > which characterizes the ferromagnetic to paramagnetic transition. In addition, one has, for this spin-1 system, a quadrupolar order parameter Q = <Si2 >. Note that the field ∆ which is conjugate to Q plays the same role as H does with respect to M. Further, the order parameters M and Q are not totally

18

A Paradigm Called Magnetism

Fig. 1.7. Phase diagram in the T – ∆ plane. For ∆ < ∆c, one has a second order transition from the para-to-ferro-magnetic phase. For ∆ > ∆c, the transition changes over into first order (dashed line).

independent of one another. For example, it is not possible to have a stable state in which M = 1 and Q = 0, since M = 1 requires that all the spins have Si = 1 which in turns leads to Q = 1. The two-order parameters are therefore kinematically coupled in the sense that even in the absence of interactions, there are constraints on the values which can be taken on by the two together. It is the competition between the two kinematically coupled order parameters which is eventually responsible for the occurrence of the tricritical point. The exchange term in Eq. (1.15) gives a lower energy for M = 1, while the crystal field term favours Q = 0. These two values are incompatible, however. The increase in ∆ ultimately makes it more favourable energetically to have Q = 0 (and hence M = 0) than M = 1. The meaning of the various phases, that are expected to occur in relation to Fig. 1.7, become clearer if one considers an applied magnetic field H in addition to the crystal field and Ising terms in Eq. (1.15). The Hamiltonian now becomes

H=−J

∑S S

iz jz

+∆

∑S

2 iz

i

−H

∑S

iz

i

.

(1.16)

An Assortment of Well-Established Concepts

19

The corresponding phase diagram, in the space of three field variables (in the sense of Sec. 1.2): T, ∆ and H, is shown in Fig. 1.8. The two-dimensional phase diagram shown in Fig. 1.7 is a projection of the three-dimensional diagram of Fig. 1.8 onto the H = 0, (T – ∆) plane. One now has a first order co-existence surface A in the H = 0 plane, on which the order parameter M assumes nonzero values with opposite signs depending on whether H → 0 from positive or negative directions, exactly as in Fig. 1.7, for T < Tc. As T increases, keeping ∆ ‘small’ the surface A terminates in a line of critical points (the bold solid line on the H = 0 plane in Fig. 1.7). However, for T < T * and ∆ > ∆*, this line of critical points terminates in the two-phase co-existence line D, which is a line of first order transitions, shown as a dashed-dotted line in Fig. 1.8. Looking at Fig. 1.8 one notes that A is connected along the line D to two first order (co-existence) surfaces B and B′ extending symmetrically into the regions H > 0 and H < 0, respectively. The surfaces B and B′ themselves terminate with increasing temperature in lines (bold solid ones) of critical points. These two critical lines (for H ≠ 0) fan out symmetrically from the H = 0 plane and join the critical line (for H = 0) at the tricritical point (the black dot). Thus, the tricritical point may be regarded either as the termination of a line (D) of triple (or three-phase co-existence) points, or equivalently, as the confluence of three lines of critical point. In fact, it is the latter feature which prompted Griffiths to name the special point a tricritical point [35]. We will return to further discussion of the phase diagram in Fig. 1.8 in the context of a very different system, viz. a He3 – He4 mixture. A model of the kind described by Eq. (1.15) has been used by Blume to explain first-order magnetic phase changes in UO2 [33]. It was found that depending on the ratio of the crystal field splitting ∆ to the molecular-field splitting (appropriate to the exchange term in Eq. (1.15)), one obtains either a paramagnetic state, a first order phase change (indicated by the dashed line in Fig. 1.7), or a second order transition (shown as the solid line in Fig. 1.7). The confluence of the first order line and the second order line, viz. the black dot in Fig. 1.7, is a tricritical point, as discussed above. While the tricritical phenomenon in UO2 takes place in the absence of an external magnetic field, first-order phase transitions are known to occur in magnets to which an external magnetic

20

A Paradigm Called Magnetism

field is applied. Such systems are known as meta-magnets. A case in point is the system of FeCl2 which belongs to a class of meta-magnets that exhibit a tricritical point [36]. The mechanism is discussed below.

Fig. 1.8. Phase diagram for an Ising magnet in the presence of a crystal field ∆ and a magnetic field H. There are three surfaces of first order transitions A, B, and B′, which meet at the tricritical point that may be viewed also as the meeting point of three lines (solid) of second order phase transitions.

In FeCl2, Fe ions are placed on stacks of parallel triangular lattices separated by Cl ions, as shown in Fig. 1.9. Each Fe ion is surrounded by a cage of six Cl ions. The iron is in the valence state of Fe2+ and carries an effective spin of one. The sign of the exchange interaction within a layer is positive, favouring ferromagnetism whereas that between layers is negative yielding anti-ferromagnetism. Further, the spins are preferentially aligned perpendicular to the layers because of lattice anisotropy. Thus, in the fully ordered state, the spins in a given plane are parallel, but they alternate in direction from layer to layer, thereby yielding a two-sub-lattice anti-ferro-magnetic order. When an external magnetic field is applied normal to the layers, the sub-lattice magnetization which is conducive to the applied field will show enhancement, whereas the neighbouring sub-lattice magnetization will undergo a decrease. Thus, there occur both a uniform magnetization and

An Assortment of Well-Established Concepts

21

Fig. 1.9. Crystal structure of FeCL2.

a sub-lattice magnetization. Again, we have a situation with two competing order parameters, like in the example discussed in the beginning of this section. When the applied field is large enough to polarize all the spins, anti-ferro-magnetic order will be destroyed. The experimental phase diagram for FeCl2, for which the uniform magnetization m is plotted along the ordinate and the temperature T is plotted along the abscissa, is shown in Fig. 1.10. When T is large and the uniform magnetization is sufficiently small we are in the anti-ferromagnetic (AF) phase. Keeping T fixed on the high temperature side and enhancing m, as can be achieved by increasing the strength of the applied magnetic field, one crosses into the paramagnetic (PARA) phase, as argued above. The line of demarcation is a line of critical points i.e. a line of second order phase transition. Below a certain temperature indicated by a black dot and labeled by Ttr, we have phase separation, meaning thereby that two phases, one with ‘large’ uniform magnetization and the other with small uniform magnetization (and concomitantly, a

22

A Paradigm Called Magnetism

‘large’ staggered magnetization), co-exist. The point Ttr is the tricritical point.

Fig. 1.10. Schematic phase diagram for the metamagnet FeCl2.

It may be noted that the phase diagram in Fig. 1.10 is in the mixed density-field variables space, in accordance with the nomenclature introduced in Sec. 1.2. Thus the portion of the diagram to the left of T * looks qualitatively like the magnetization versus temperature diagram of an ordinary ferro-magnet. Had we drawn the phase diagram in the field variables space by replacing the magnetization by its conjugate magnetic field the two-phase co-existence region would have shrunk to a first order line, meeting the second-order line at the tricritical point, as in Fig. 1.7. A very similar phenomenon of tricritical points is found in a completely different system of a binary mixture of He3 and He4 in which He4 can occur in two different phases: normal and suverfluid, the two phases being related by a symmetry operation. Indeed a slight modification of the Hamiltonian as employed in Eq. (1.16) for the metamagnet FeCl2 goes under the name of the Blume-Emergy-Griffiths (BEG) model that was used for describing the tricritical point in He3 – He4 mixtures [37]:

23

An Assortment of Well-Established Concepts

H = − J ∑ Siz S jz − K ∑ ( Siz )2 ( S jz )2 + ∆ ∑ Siz 2 − H ∑ Siz . (1.17) < ij >

< ij >

i

i

Under saturated vapour pressure it is observed that the superfluid %-transition temperature decreases with increasing mole fraction x of He3, and below a temperature & ' 0.87* corresponding to 0.67, a first order phase separation takes place (Fig. 1.11).

Fig. 1.11. Phase diagram (schematic) for /5 6 0 /5 7 mixtures. The two-fluid coexistence curve is labeled D, the dashed curve is the line of the lambda transitions and the dot indicates the tricritical point.

The corresponding phase diagram in the space of field variables is the same as in the case of the metamagnet FeCl2 (Fig. 1.8) in which ∆ may be interpreted as the themodynamic field conjugate to x, i.e., ∆ is the difference in chemical potentials of He3 and He4, and H is a fictitious field conjugate to the superfluid order parameter .. The first order coexistence surface A in the / 0 plane extends to ∆ 01 (pure He4). On A, . assumes nonzero values with opposite signs, as described earlier following Eq. (1.16). Thus . is the analog of the magnetization M, the order parameter in the magnetic case. The BEG model has a built-in time-reversal symmetry (in the absence of H) with the consequence that odd terms in the spin operator 234 , for instance, are absent. The most general spin-one model however, which subsumes the BEG model, Eq. (1.17), and the Hamiltonian for the metamagnet, Eq. (1.16), does not have to obey this symmetry, and is

24

A Paradigm Called Magnetism

therefore, applicable to a ternary liquid mixture. The corresponding Hamiltonian can be written as [38]:

08 9 234 2;4 0 * 9 234 = 2;4 = 0 > 9 234 = 2;4 :3;

is independent of the site index j. Therefore H i ≡ H = J (0) < S z >, where z

J (0) = Z J ij .

(2.4)

Hi = −( HS zi + ΓS xi ).

(2.5)

j =1

Hence, Eq. (2.2) yields

The partition function is given by

ƕ( %012 3 4 56Ɩ 7 869 :,

2.6

where < = %& . Because S z takes only two discrete values +1 and −1 we can use properties of 2x2 matrices to decompose the exponential operator in Eq. (2.6), in order to simplify ƕ( as

Z i = 2 cos ℏ (βh ),

(2.7)

independent of i and where

h=

H 2 + Γ2 .

(2.8)

Thus

< S z >=

1 Tr [ S zβ ( HJ z + ( ΓS x ) ], 2 cosh( β h )

(2.9)

which yields

< sz >=

H tanh( β h). h

(2.10)

34

A Paradigm Called Magnetism

Similarly,

< S x >=

Γ tanh( β h). h

(2.11)

Denoting the LHS of Eqs. (2.10) and (2.11) as the components of the magnetization mz and mx respectively, we obtain the transcendental equations:

mz =

mx =

J (o ) m z

tanh( β ( J (o ) mz ) 2 + Γ 2 ),

(2.12)

Γ tanh β ( β ( J (o)mz ) 2 + Γ 2 ). ( J (o ) mz ) 2 + Γ 2

(2.13)

2

( J (o) mz ) + Γ

2

The above equations yield self-consistent relations for the two relevant magnetization components. Note that the order parameter mz vanishes when either Γ or T goes to infinity. This confirms our earlier physical argument that Γ acts as a disordering field. We may now discuss the phase diagram predicted by Eqs. (2.12) and (2.13) by designating the order parameter mz as ψ and defining the critical temperature for the pure >. . ? 0 Ising model as

Tco =

J (o ) kB

(2.14)

Equation (2.12) then yields (for the solution corresponding to ψ ≠ o )

o 2 T 1= tanh c ψ + Γ 2 , T Tco ψ / T )2 + Γ 2 Tco / T

(2.15)

where Γ = β Γ. At the phase boundary, ψ = o, thus leading to

$

TBC tanh?I$ , 8DB

2.16

Quantum Phase Transition: Transverse Ising Model and Other Systems

35

which is equivalent to

Γ Γ = tanh . J (o) K BTc

(2.17)

The corresponding phase diagram is shown in Fig. 2.1 demarcating the following three regimes:

Fig. 2.1

Region I, where Γ is large, and T is small – quantum effects are dominant here. Region II, where Γ is small – classical effects are dominant and the TIM is analogous to the usual Ising model. Region III, where both Γ and T are moderate. We next analyze the static susceptibility in region III, by adding a small aligning field ∆H along the Ƶ-axis. In that case, Eq. (2.15) can be rewritten as

36

A Paradigm Called Magnetism

ψ=

β∆H + Tco

ψ

ψ tanh ( β∆H + Tco T ) 2 + Γ 2 . ψ ( β∆H + Tco T ) 2 + Γ 2 T

(2.18) Linearzing in ψ and ∆H leads to

Tc0 tanh tan ℏΓ ψ 1 − = β∆H , 2 T Γ Γ

(2.19)

yielding for the susceptibility −1

ψ tan Γ tan Γ χ= = T − Tc0 . ∆H kBΓ Γ

(2.20)

Thus, χ diverges at the critical temperature Tc given by Eq. (2.16) with a mean field critical exponent K 1. Alternatively, χ can be rewritten as

χ = tanh Γ(Γ − KBTco tanh Γ)−1 ,

(2.21)

which again shows a divergence at the critical value of the transverse field Γ = Γ c given by Eq. (2.16) with the same exponent K 1.

2.3. The Quantum Magnet LiHoF4 The system LiHoF4 belongs to a class of compounds LiRF4 , where R is a rare earth element (Fig. 2.2). Although the rare earth elements of Ho 3 + in LiHoF4 are coupled by dipole-dipole interaction, only the lowest doublet of the 17 crystal-field-split states is appreciably populated at low temperatures (T < 2 K ) because of a large crystal field. Further, the sign of the crystal field is negative; hence the lowest doublet corresponds to the highest spin states. Consequently, the off-diagonal terms of the dipolar interaction are effectively “quenched” leading to the so-called “truncated dipolar Hamiltonian” [45]. The latter is of the Ising

Quantum Phase Transition: Transverse Ising Model and Other Systems

37

Fig. 2.2. The Crystal structure of LiHoF4.

type, yielding an Ising coupling between spins projected along the crystallographic c-axis, with the interaction J ij of the form:

1 − 3cos 2 θ ij J ij = J , rij3

(2.22)

where θ ij is the angle between the Ising axis (i.e. the c-axis of the crystal) and the position vector connecting the spins. As seen in −3 Eq. (2.22), J ij is very long-ranged because of its rij dependence on the inter-spin distance rij . This indicates that a mean-field treatment will be in order for such a system. However, the angular dependence [1 − 3cos2 (θij )] allows for J ij to change sign, implying that the interaction switches from ferromagnetic ( J ij > o) to antiferromagnetic While this ( J ij < 0) for intermediate angles (55 ≤ θij ≤ 125 ) . occurrence of competing interactions may raise doubts about the uniqueness of the ground state, a classic analysis by Luttinger and Tisza [46] demonstrates that the ground state is indeed that of a dipolar ferromagnet for the b.c.c structure of LiHoF4 . The experimentally measured critical temperature for the paramagnetic – ferromagnetic transition turns out to be Tc = 1.53K . Having arrived at a situation in which one has an Ising model as an approximate low-temperature description of the dipolar-coupled system,

38

A Paradigm Called Magnetism

the question arises: How does one realize a TIM? In the experiment of Bitko et al. [47], a small magnetic field H t transverse to the c-axis is applied in the laboratory which causes admixture of the two eigenstates of the crystal-field-split doublet (See Fig. 2.3), yielding (in perturbation theory) a spin Hamiltonian that is proportional to S x , with a prefactor Γ∞H t2 . Thus, single crystals of LiHoF4 provide a clean model system in which high-precision, controlled investigation of quantum critical phenomena can be performed. In one other aspect, LiHoF4 is unusual in that the observed magnetic behavior is quantitatively described by mean-field theory, discussed in Sec. 2.2 [48]. The fact that the quantum critical behavior in d = 3 is mean field-like is not surprising as it is known that the d-dimensional quantum phase transition (at T = 0) for the TIM is equivalent to the ( d + 1) dimensional thermal phase transition for the ordinary Ising model [49, 50]. The mean field nature of the thermal phase transition observed in LiHoF4 is also not surprising as renormalization group (RG) theory shows that, for a dipolar-coupled Ising system, the marginal dimensionality is L$ 3, barring logarithmic corrections for critical exponents. [51]. (Recall that we expect mean field behavior for d > d c .) We now bring-in one additional attribute of the LiHoF4 system that is crucial for a satisfactory understanding of the experimentally observed phase diagram, especially at low temperatures. The ionic spin of Ho3+ element has a non-negligible hyperfine interaction with the nuclear spin of Ho in which the coupling constant is of the order of 0.039K. Because the large crystal field ‘quenches’ the off-diagonal terms of the spin operator of Ho3+ (with the crystallographic c-axis as the direction of quantization), as mentioned before, the hyperfine interaction is also axial [48]. Incorporation of this interaction generalizes the Hamiltonian in Eq. (2.1) to: N

N

H = −∑ J ij Siz S jz − Γ∑ Six − a∑ Iiz Siz ,

i =1

i =1

(2.23)

Quantum Phase Transition: Transverse Ising Model and Other Systems

39

where ‘a’ is the hyperfine coupling constant and I iz is the nuclear spin of the ith Holmium nucleus. Correspondingly the single site mean field Hamiltonian in Eq. (2.2) has to be generalized to:

Hi = −[( H i + aI zi ) S zi + ΓS xi ].

(2.24)

With the Hamiltonian in Eq. (2.24) we now proceed to evaluate the phase diagram [52]. In accordance with our earlier analysis the partition function for a single site in the mean field approximation can be written as

ƕ 34 57MNO 6P7869 :,

2.25

independent of i and in which the trace is over the ionic as well as the nuclear spin eigenstates of Ho. Labeling the 8 nuclear eigenstates by |S , we have TƖ |S S|S where M assumes values – 7/2, -5/2, ………5/2, 7/2. Thus +7/2

Z=

∑

2 cosh β h( M ),

(2.26)

( H + aM ) 2 + Γ 2 .

(2.27)

M =−7/2

where h(M ) =

Proceeding as before, Eq. (2.12) for the order parameter can be written as

∑[ mz =

M

aM + J (o ) mz ]Sinh ( β h ( M )) h( M ) . ∑ cosh( β h( M ))

(2.28)

M

The phase boundary shown in Fig. 2.3 is estimated from a numerical solution of Eq. (2.28). The solid curve drawn through the dots is merely a guide to the eyes. The dashed line is the phase boundary in the absence of hyperfine interaction, as shown also in Fig. 2.1. The inset shows the experimentally obtained phase boundary of Bitko et al. from susceptibility measurements (filled circles) and the calculated mean-field phase boundary (solid line) in the presence of hyperfine coupling

40

A Paradigm Called Magnetism

from an 136 x 136 eigenfunction space of the full Hamiltonian (nuclear spin = 7/2, ionic spin = 8) [48]. The dashed line in the inset is the result of computation in the absence of hyperfine interactions. The deviation of the phase boundary from the dashed line for high values of the transverse field Γ can be understood from the following physical considerations. For small Γ the local mean-field is dominated by the effective Ising interaction proportional to the magnetization along the c-axis. However, as Γ increases, the magnetization along the c-axis goes on decreasing (because of the gradual loss of the quantization axis) leading to the situation in which the local field is totally dominated by the hyperfine coupling alone. Because it is the competition between the local field and the transverse field that determines the phase boundary between the ferromagnetic and paramagnetic phases, the ferromagnetic order persists for a larger values of the transverse field, especially at low temperatures, since the hyperfine field takes over the role of the local mean field. This analysis is in conformity with the experimental observation of Bitko et al. in that there is an upward tilt in the phase boundary for temperatures lower than 0.6K [48].

Fig. 2.3. The crystal field splitting in LiHoF4, indicating that at ultra low temperatures, one has an effective 2-state model.

Quantum Phase Transition: Transverse Ising Model and Other Systems

41

2.4. Quantum Statistical Mechanics With the preceding background to quantum phase transition (QPT) in the context of an example borrowed from Magnetism we turn now to the general statistical mechanics discussion on why a QPT is so different from its classical counterparts. Note that the main issue in evaluating the partition function in statistical mechanics concerns the diagonalization of the Hamiltonian. Once this is done one can choose to work in a representation in which the Hamiltonian is diagonal and then compute the trace of the density operator %41 merely in terms of the eigenvalues of H , for completing the calculation of the partition function. The reason this task is difficult in general in a quantum problem is evident from the example of the transverse Ising model; the Ising term is diagonal in the representation of the spin operator , , while the transverse term is diagonal in the representation of the spin operator S x ! Thus there is no definite axis of quantization and hence, the task of diagonalization is humongous, barring the special case of one dimension, or finite systems. This problem is of course peculiar to quantum mechanics because in classical statistical mechanics the kinetic energy and potential energy terms (which add up to the Hamiltonian H ) can be dealt with separately. The term in the partition function involving the kinetic energy yields a Gaussian integral over the momentum variable that leads to a simple temperature – dependent prefactor and all the many body effects are subsumed in the potential energy term. Not that it always leads to a happy situation as far as an exact calculation of the partition function is concerned, as we very well know from the examples of the ordinary Ising model in three dimensions, or interacting classical liquids, etc., but the first battle is won, viz., the kinetic and potential energy terms can be disentangled. Indeed it is this attempt towards disentanglement that yields the basis of the Feynman’s path integral formulation of the partition function, as discussed below [53]. The partition function in the canonical ensemble can be written in terms of a summation over a complete set of states:

U < ) WX %41 XW . V

2.29

42

A Paradigm Called Magnetism

Note that the density operator %41 is identical to the timedevelopment operator e −iHτ /ℏ , if the time τ is considered to be imaginary: τ = −it β . Thus Z is the sum of transition amplitudes for the system to start from some state f > and return to the same state f > after a time interval − iℏ β . The total time interval, which is fixed by temperature, will naturally be infinitely long (along the imaginary axis) at 0! The idea of Feynman is to break up the net transition amplitude between the states of a system into a series of transition amplitudes over intermediate states and summing over all possible paths between the two states. The path in question is defined by specifying the state of the system as a sequence of finely spaced intermediate time steps. One may formally write

e − β H = [e

1 − δτ H N ℏ

] ,

(2.30)

where δτ is a small time interval given by δτ = ℏ where E is taken to E be larger than the highest energy scale in the problem, and N is an integer chosen such that N δτ = ℏ β . We now use the Trotter identify [54]: d c

d

[\ ]^ _>` a a a ,

2.31

ab∞

where [\ and ]^ are two bounded quantum operators. Writing H as H = Τ + V , where T is the kinetic energy operator and V the potential energy operator, the kinetic and potential energy terms can be disentangled in the limit e b 0. Hence the idea of employing a small time interval δτ is to enable the use of classical-like methods by ignoring the non-commulativity of T and V over the small time segment δτ ! Using a succession of closure property the partition function may be rewritten as

U < ) )

&

V Vj Vk …Vm

x < f1e

1 − δτ H ℏ

W f %ghi5 f W&

| f 2 >< f 2 | .... | f N >< f N | e

1 − δτ H ℏ

| f >.

(2.32)

Quantum Phase Transition: Transverse Ising Model and Other Systems

43

j

Note that a typical matrix element such as W& n %ghi5 n Wo signifies an amplitude of transition (in imaginarily time >e from the state |W& to the state |Wo . This is reminiscent of a transfer matrix that connects one site to another in classical statistical mechanics of the Ising model, for instance [17]. Therefore, in the present case, the imaginary time may be thought of as an extra spatial dimension. This indeed is the reason why the statistical mechanics of a d-dimensional quantum system can be viewed equivalent to a ( d + 1) − dimensional classical system, except that the extra dimension is finite in extent, going to infinity only at T = 0 . The underlying idea can be illustrated in terms of the following physical example.

Fig. 2.4. Josephson junctions (crosses) demarcating superconducting grains.

Consider a one-dimensional array of Josephson junctions shown schematically in Fig. 2.4 [44]. The crosses indicate junctions between superconducting grains. Over each grain the superconducting state is characterized by a condensate wave function. Josephson tunneling of cooper pairs from one grain to another occurs across the junctions. The order parameter at hand is the condensate wave junction itself which iθ for the j th grain can be written as ψ j = a j e j . As it turns out it is the fluctuations of the phase angle θ j that are relevant while those of the amplitude a j can be ignored. Because tunneling involves overlap of the wave function between grains, the corresponding interaction Hamiltonian is proportional to the projection operator |p+ p+7& | between the j th and its neighboring ( j + 1) th grains. If coherence of the wave function is maintained, tunneling is facilitated and the system (i.e. the one-dimensional array) is super-conducting. This process however is

44

A Paradigm Called Magnetism

counter balanced by the energy required to transport an excess cooper pair onto a grain, i.e. the coulomb repulsions between pairs. If this energy is large, especially for small grains, the Cooper pairs will be blockaded and the system becomes an insulator. It is this superconductor-insulator transition which is the underlying QPT in the present instance. Given this background the Hamiltonian for the Josephson junction array can be written as:

1 o 1 )q^+ ) r+ stu^+ u^+7& , 2 +

+

2.33

where the hat over a dynamical variable the phase angle signifies its operator nature, E j is the Josephson coupling strength, C is the intra-

grain capacitance and q^+ is the ‘voltage operator’ for the j th grain. Λ

Because q^+ is conjugate to the dynamical variable θ it has a differential j

operator form (analogous to the co-ordinate representation of the momentum operator in quantum mechanics): Λ 2e ∂ . V = −i j C ∂θ j

(2.34)

(Note that the extra factor of 2 in front of e accounts for the total electric charge of a Cooper pair). Substituting Eq. (2.34) in Eq. (2.33) the Hamiltonian can be rewritten as

H = − Ec ∑ j

Λ Λ ∂2 − ∑ E j cos(θ − θ ), 2 j j −1 ∂θ j j

(2.35)

where

Ec =

2e 2 . C

(2.36)

The first term in Eq. (2.35) is analogous to the kinetic energy of a rotor where Ec−1 is like the moment of inertia.

Quantum Phase Transition: Transverse Ising Model and Other Systems

45

At this stage it is possible to draw an analogy between the Hamiltonian in Eq. (2.35) and that of the TIM (cf., Eq. (2.1)). The Josephson energy is akin to the pure Ising coupling in that each interaction favors ‘order’ be it in the form of preserving the phase coherence of the condensate wave function or ferromagnetism respectively. The charging energy, proportional to E c is like the transverse term Γ of TIM that has the effect of disrupting order by effecting quantum transitions between the eigenstates of the angle Λ

operator θ (or the spin operator S jz , in the TIM case). Understandably j

then, the disordering field or the control parameter for the quantum phase transition in the Josephson junction array is expected to be proportional to the ratio of E c and E j . (For a precise relation, see below). When this ratio exceeds a certain critical value the system transits from the superconducting to the insulating phase. As discussed before in the context of the expression for the partition function (Eq. 2.32), each transition amplitude < f1 | e

1 − δτ H ℏ

| f2 >, which

is a statistical weight of a space time path, is the Boltzmann weight of the classical configuration for an equivalent 2d-classical model, in which the extra dimension is along the imaginary time axis. The latter turns out to be the 2-dimensional classical XY-model, the Hamiltonian of which has already been introduced in Eq. (1.3). The angles θ i are now to be interpreted as those of planar spins that lie on a two-dimensional square lattice. It turns out that the coupling constant J is proportional to E J / EC . The inverse of J is then a ‘fake’ temperature for the model, the increase of which causes the coherent ordering of the phases (for the original model) to disappear. On the other hand, a large value of J makes it unlikely that the angles θ i and θ j will differ significantly, even when the sites i and j are far apart (in space and/or time), yielding a superconducting phase. We should emphasize that this equivalence between the one-dimensional Josephson junction array and the twodimensional classical XY-model is only in the sense of universality near the corresponding critical points (cf., Chapter I). Other than that

46

A Paradigm Called Magnetism

however the underlying proof of equivalence goes over to d-dimensional arrays and ( d + 1) − dimensional classical XY models. This is a very useful result in that numerical methods such as Monte Carlo techniques can be applied to study the critical behaviour of d-dimensional quantum models. In conclusion, we note that all the basic ideas of quantum phase transitions and the concomitant quantum critical points have not only a historical connotation to Magnetism but are also most easily understood within the context of a magnetic model eg. the transverse Ising model. Further details of zero temperature (T = 0) dynamic scaling, finite-size scaling for T ≠ 0, and Quantum Hall Effect as a prototypical experimental system of QPT can be found in the eminently readable review article of Sondhi et al. [44].

Chapter 3

Glass Transitions 3.1. Preamble Magnetic Glass, Quantum Glass, Spin Glass, Proton Glass and Structural Glass One of the enigmatic unresolved issues of the contemporary materials physics is the glass transition. The problem is simply stated in the context of an ordinary, monatomic liquid. When the latter is cooled very slowly, i.e. adiabatically such that at every stage of the cooling process the liquid is in thermal equilibrium with the heat bath in which it is embedded, it usually freezes into a crystalline solid at a temperature TF. However, when the liquid is rapidly cooled, i.e. supercooled, it solidifies into a disordered amorphous structure called glass, which has no translational or orientational symmetry unlike a crystal. The transition temperature TG ( TB leads to paramagnetic response which is Curie like (T −1 ) whereas T < TB blocks the magnetization. Polydispersity (i.e., size distribution) will of course cause a broadening of the hump. 5.3. Experiments: Stern–Gerlach and Mössbauer Spectroscopy With the introductory background to the phenomenology of singledomain nano-magnetic particles and the underlying relaxation theory we turn our attention in this section to experimental measurement of the relevant properties. The parameters of interest which can be extracted from experiments are: a) b) c) d)

size or volume V of the particles; the magnetic moment per unit volume µ; the anisotropy energy K, which provides the barrier to relaxation; polydispersity, viz., the distribution function that characterizes the size-distribution, if there is any; e) and interparticle interaction, the most commonly encountered one being the dipolar one. We have so far ignored (e) and considered only independent, noninteracting magnetic particles, and the only measurement techniques we have touched upon in passing are the magnetization and the susceptibility. In what follows, we shall examine a variant of the celebrated Stern-Gerlach setup that has been recently used to study relaxation of nanomagnetic particles, especially magnetic clusters [117].

118

A Paradigm Called Magnetism

Magnetic Clusters in a Stern-Gerlach Setup The experimental configuration is shown in Fig. 5.9. The only difference with the historic experiment is what are jettisoned from the oven are not singly charged Ag ions but single-domain clusters of Co, Gd, etc. For a cluster whose magnetization µV is polarized along the direction z of the inhomogeneous magnetic field one would have expected in the old measurement that the deflection d on the detector screen, measured from z = 0 , would be given by

d=

µV M

B ′ (o )

LD L (1 + ), 2 v 2D

5.63

where m is the mass of the particle, is the gradient of the magnetic field B(z) at z = 0, v is the (constant) speed with which the jet emanates from the oven in the forward (i.e. normal to z-axis) direction and the Length L and D are defined in Fig. 5.9.

S

Fig. 5.9. Stern-Gerlach Setup.

The first contribution within the round brackets in Eq. (5.63) comes from ballistic motion outside the magnet while the second term arises from the accelerated motion within the magnet. Though Eq. (5.63) is wrong in the present discussion because of rotational relaxation of the cluster magnetization within the magnetic pole-pieces region, as will be shown below, it allows for the introduction of an important parameter GS that defines the experimental time-window for the setup at hand:

119

Memory in Nanomagnets

τE ≡

5.64

L . v

The reason Eq. (5.63) is wrong is that the velocity v¡ of the cluster, derived from the acceleration gained in the z-direction in view of the force exerted by the inhomogeneous magnet on the magnetic moment of the cluster, is now a stochastic process, given by P

v¡ ¢ cos , 3

(*

5.65

where ¢ is a constant parameter of the experiment: ¢ ¤ ¥ and θ (t ) is the angle between the magnetic field (i.e. z-axis) and the magnetization vector of the particle. For reasons discussed in detail in Sec. 5.2 the relaxational dynamics of cos θ (t ) may be described in terms of the Fokker-Planck equation (5.25). We would like to dispose of one red herring in order to facilitate comparison with experimental data. Note that the initial conditions chosen on v¡ is that it is zero at time t = 0 , implying that the molecular jet is unidirectional. However, while this is predominantly so, there is a small residual fluctuation in the velocity in the z-direction due to the temperature Ts of the source i.e. the oven. That is, over and above the very large speed of the jet along the dashed line in Fig. 5.9, there is an envelope of velocity distribution governed by a Maxwellian at temperature Ts, thus P

where

v¡ ∆v¡ & ¢ cos , 3

< (∆v z ) 2 >=

k BTs . m

5.66 5.67

120

A Paradigm Called Magnetism

Fig. 5.10. Line profile, even at zero field, implying that there is a transverse fluctuation in velocity.

This fact is borne out in the experimental data shown in Fig. 5.10 which indicates that even for zero magnetic field (and its gradient) there is sizable broadening of the deflection profiles. This residual broadening, established from Eq. (5.67), is then added to all the theoretically computed line profile below, for a meaningful comparison with data. This discussion then also brings to fore the existence of two distinct temperatures in the problem: the oven temperature v already mentioned, which determines the jet-speed, and the lattice or the vibration temperature ¨ that governs the rotational relaxation of the magnetization of the cluster, as it tries to equilibrate to its own lattice through spinlattice relaxations. It is v that enters the discussion of the Fokker – Planck equation (5.25). (For a more detailed discussion on Ts and v see [117]). With the preceding background to the Stern-Gerlach geometry, the deflection d on the detector screen, measured from z = 0 (and upon ignoring ∆v¡ in Eq. (5.65)) can be written as ª«

ª«

3

3

P

¢© cos & ¢ cos . v 3

5.68

Clearly, d itself is a driven stochastic process, the mean value of which has to be computed from the expression (5.27), and the Kramers’

Memory in Nanomagnets

121

solution for the probability function P (θ , t ). that [118]

We have found earlier

R

¢© 1 ¢ 1 3 ¬ #GS 1 t®¯ª« ° & 1 t®¯ª« °'± ¢ z ©z z

1 © v 1 &¢ cos ¬ GSL & 1 #GS 1 t®¯ª« °'± . 2 v ©z z

5.69

where z is the Kramers’ relaxation rate that depends on the barrier height (anisotropy energy) and also the possible presence of a homogeneous component of the magnetic field in the Stern-Gerlach setup, < cos θ > eq is given by Eq. (5.4) and , is the initial polarization of the entering jet. Note that in the static limit z 0, applicable to the original Stern-Gerlach experiment, and for a fully polarized beam , 1, Eq. (5.69) reduces to Eq. (5.63), as we had anticipated earlier. The first step towards calculating the line profile, i.e., the intensity of ‘hits’ on the detector versus the deflection, requires the variance of the deflection. For computing the latter we want to evaluate the correlation function: < cos θ (0) cos θ (t ) >, which has been the subject of our earlier discussion (cf., Eq. (5.43)). But, now, cos is nonzero. We find 0cosθt

L 3 t®¯³ & ´3 1 t®¯³ °.

5.70

µµµL and from that, the variance The Eq. (5.70) is needed to compute L L µµµ R °, employing Eq. (5.69). While the variance is just the second comulant of the probability distribution of the deflection π ( d ) , in principle, all higher order cumulants are required to calculate the intensity profile. We find incredibly though that the second cumulant suffices i.e. the probability function π ( d ) is nearly a Gaussian [119]. The comparison with experimental data for Gd, and Co clusters is shown in Fig. 5.11 and Fig. 5.12 respectively. Figure 5.13 is a depiction of the intensity profile for Gd22 clusters which seems to point to a bidisperse

122

A Paradigm Called Magnetism

Fig. 5.11. Line profile for Gd23 and Gd22 clusters.

Fig. 5.12. Line profile for co-clusters, in zero and finite magnetic fields.

123

Memory in Nanomagnets

−4

−2

0 2 4 Deflection(mm)

6

8

Fig. 5.13. Double Gaussian profile for Gd22 indicating that there is a bi-modal size distribution.

distribution of sizes in the sample concerned. Thus we have a superposition of a set of clusters whose magnetization is frozen (τ > τ E ) and another set that exhibits superparamagnetism (τ < τ E ) . Mössbauer Relaxation of NiFe2O4 in SiO2 Matrix In this subsection we describe Mössbauer spectroscopy of single-domain nanomagnetic particles of NiFe2O4 embedded in a nonmagnetic SiO2 host. The samples are prepared by standard sol-gel techniques and are characterized by X-ray diffraction (XRD) and transmission electron microscopy (TEM) [120]. A rough description of three different kinds of samples used is shown in Fig. 5.14. The Table 1 below provides the relevant parameters:

124

A Paradigm Called Magnetism

Fig. 5.14. A schematic of sample sizes and their inter-particle separation.

Table 1 Sample Characteristics Average particle size Average inter-particle distance

Sample 1

Sample 2

Sample 3

3 nm

3 nm

15 nm

5 nm

15 nm

15 nm

In all cases the particle-size is found to follow a long-normal distribution which has the known attribute that dispersion goes hand in hand with the average size. Thus sample 3 with average particle size 15 nm is also expected to have the most pronounced dispersion compared to sample 1 and 2. We estimate that for sample 1, the interparticle dipolar interaction is the strongest because the average separation is about 5 nm. On the other hand, dipolar coupling is indeed very weak, for samples 2 and 3. Thus, sample 1 will be notionally referred to as “Interacting” while samples 2 and 3 as “Noninteracting”. This nomenclature is borne out by the room temperature hysteresis data, shown in Fig. 5.15. At room temperature the Neel relaxation is expected to be extremely rapid (cf. Eq. (5.11)) but the difference in the hysteresis curves for samples 2 and 3, in which sample 2 shows no hysteresis but sample 3 exhibits weak hysteresis, is precisely due to the size difference.

Memory in Nanomagnets

125

Fig. 5.15. Hysteresis behavior for samples 1, 2 and 3.

The 15 nm sized sample 3 has its relaxation time somewhat elongated (cf. Eq. (5.11)) compared to the 3 nm sized sample 2, and therefore, sample 3 requires a somewhat longer time to reach equilibrium. On the other hand, there is moderate hysteresis for sample 1 even though the average particle size 3 is the same as for sample 2; the reason is the dipolar interaction. For sample 1, the average interparticle separation is 5 nm and hence, the dipolar coupling, which is inversely proportional to the cube of inter-particle distance, is estimated to be stronger than in sample 2, again slowing down relaxation. In order to focus onto the effect of inter-particle interaction, keeping the average size fixed, we show temperature-dependent Mössbauer spectra in Fig. 5.16 for sample 1, and Fig. 5.17 for sample 2. The data at 20 K for both samples exhibit the characteristic six-finger pattern for 57Fe, contained in NiFe2O4, although sample 2 displays slight broadening of lines, implying that relaxation is not completely frozen, even at 20 K. As the temperature increases, relaxation speeds up and for sample 2 and at room temperature (RT), complete ‘motional narrowing’ sets in, yielding a single absorption line. Evidently, this speeding up of relaxation is not adequate for sample 1 which, even at RT, demonstrates

126

A Paradigm Called Magnetism

a split-lineshape. This effect is again attributed to the more pronounced dipolar interaction for sample 1 which competes with thermal energy in modulating the relaxation time scales. Thus, within the Mössbauer time window, which is nearly 10-8 sec corresponding to the lifetime of the excited nuclear state, the magnetization is apparently frozen for sample 1, even at room temperature! Relaxation Theory Within a Two State Model We have seen earlier that because of thermal fluctuations the magnetic moment undergoes rotational Brownian motion over an anisotropy barrier, in which the angle between the anisotropy axis and the magnetic moment vector is a continuous stochastic process. However the Kramers’ analysis showed that when KV>>kBT (in reality though KV can be a few times larger than kBT in order that the Kramers analysis is valid), the magnetic moment is mostly locked-in two orientations

0 and [, with slow relaxation between the two configurations. We are thus in the so called “Ising’ limit in which may be viewed as a dichotomic Markov process, in which it jumps at random between the angels 0 and [ at a rate given by the Arrhenius – Kramers formula (Eq. 5.10) (cf., also Fig. 4.1).

Fig. 5.16. Mössbauer lineshape for sample 1. Even RT spectre show split lines.

Memory in Nanomagnets

Fig. 5.17. Mössbauer spectre for sample 2. narrowing’.

127

The RT spectrum indicates ‘motional

We now discuss in somewhat more detail the effect of dipolar interaction. The latter is well known to yield complex magnetic order, being long-ranged, anisotropic and alternating in the sign of interaction. However, our hysteresis measurement, exhibited in Fig. 5.15, indicates that even for sample 1 for which the dipolar coupling is relevant, there is no shift of the hysteresis loop, thereby implying that the bulk magnetization, for the zero applied field, is zero. Our interpretation is that because of the largeness of the anisotropy barrier ¸ K we are in the Ising limit of the dipolar interaction, for which the local field, in the mean field sense, points parallel or antiparallel to the anisotropy axis, with equal probability. The dipolar interaction can now be described by its truncated form: ¹{t{

1 3 L º r Z Zº » ·¡ ·¡º , |¼º |½ º

L

5.71

where Z and Zº are the gyromagnetic ratio of the ith and jth particles respectively, WWWX ¼¾¿ is the vector distance between the sites at which the particles are located, º is the angle between the WWWX ¼¾¿ and the anisotropy axis and mzi is the (giant) magnetic moment for the ith nanoparticle along the anisotropy axis (i.e. Z). Given that m ¸ V, Eq. (71) may be rewritten as

128

A Paradigm Called Magnetism

¹{t{ L L r Z Zº »L º

1 3 L º º . ½ |¼WWWX ¾¿ |

5.72

Further, we assume the validity of mean field theory in which each nanomagnetic particle is imagined to be embedded in an effective medium that creates a local magnetic field at its site. The mean field (MF) form of Eq. (5.72) is ¥À ¹{t{ Z»L L r Zº » º

1 3 L º º , ½ |¼WWWX ¾¿ |

5.73

where the angular brackets < …. > represent a thermal average. Further, in accordance with our assumption about the largeness of the anisotropy energy, can be replaced by a two-state Ising variable Á: ¥À ¹{t{ Z»L L Á r Zº » º

1 3 L º Áº . ½ |¼WWWX ¾¿ |

5.74

In line with this approximation each particle can be viewed to be subjected to a local magnetic field H such that ¥À Á, ¹{t{

5.75

ÂÃ Á ,

5.76

ÂÃ ]" . k

5.77

where Â is a parameter that subsumes all the other constants. Within the proposed mean field theory, H can be expressed as (cf., Eq. (5.7))

Note that Eq. (5.77) admits both positive and negative solutions for H, in accordance with out discussion preceding Eq. (5.71). We now turn our attention to relaxation kinetics. Within the previously stated physical picture in which the Fokker-Planck process is replaced by a dichotomic Markov process we may write down the following set of rate equations for the number of magnetic particles with a specific orientations of their magnetization:

129

Memory in Nanomagnets

" Ä32 "3 &Ä23 "2 , 3 " Ä32 "3 Ä23 "2 , 2

5.78 5.79

where the subscripts on n indicate the two allowed values of . Solving Eqs. (5.78) and (5.79) we may derive for the time-dependent magnetization M(t): "3 "2

Å & 0 Ä

ΔÄ Å , 1 Ä Å Ä

where ", & "2 is normalized to unity, Å Ä32 &Ä23 , Ä

and

∆ Ä λ23 λ32 . GÇtM

GttM

5.80 5.81 5.82

Here Ä32 equals whereas Ä23 equals (cf., Eq. (5.11)). Furthermore, note that if M(t = 0) equals zero and ; K (linear response considered) Eq. (5.80) yields the earlier written expression in Eq. (5.12) wherein , is given by a combination of Eq. (5.3) and Eq. (5.7). Thus in the ‘high barrier – weak noise’ Kramers limit the two-state rate theory yields completely equivalent results as can be independently obtained from the Fokker-Planck description. Interpretation of the Mössbauer Spectra

The Mössbauer data shown in Fig. 5.16 and Fig. 5.17 are interpreted on the basis of the following stochastic model Hamiltonian: ¹ È ÉÊÊ¡ ,

5.83

where È is the nuclear magneton, g(I) is the level-specific g-factor ½ depending on whether the 57Fe nucleus is in its excited state I = L or the M L

ground state I = , Ê¡ is the component of the nuclear angular momentum

130

A Paradigm Called Magnetism

along the anisotropy direction, and h(t) is a local field at the nucleus that jumps about stochastically in time. The local field h(t) at the nucleus is of course produced by the magnetization of the particle which, for reasons outlined earlier, is taken to jump between Ë, , where , is proportional to H, given by Eq. (5.77). The rates at which these jumps occur are given by Ä32 and Ä23 . The Mössbauer lineshape as a function of the frequency is then given by [121, 122]. Ê

1 Ì r | Ê3 ·3 |Í |ÊM ·M |L [ ~ ~Î

tM

L L Ð È 3 É3 ·3 ÉM ·M L x Ï! & & Ñ Å Ä Ð 2 :! & 2< & 2

.

5.84

In Eq. (5.84) Í is the nuclear transition operator, the matrix elements of which are given by Clebsch-Gordan coefficients, Ð is the natural linewidth of the excited level, g’s are the ground and excited level g-factors Å is the volume-dependent rate given by Eq. (5.81). The and Ä integral over V incorporates the particle size distribution with the aid of a probability function f(V). As we mentioned earlier in connection with Fig. 5.15, the spectra are indicative of the presence of an apparently static magnetic field which is an internal field due to the dipolar interaction. The significant feature of the dipolar coupling is that the mean field H occurring in the exponent of the relaxation rates Ä32 and Ä23 is itself volume-dependent (cf., Eq. (5.77)). Therefore, the relaxation rates acquire an additional V2dependent term in the exponent, for the ‘Interacting’ sample 1. Thus, λ for a given temperature is systematically smaller for the interacting case (sample 1) than for the noninteracting case (sample 2). Hence, even at the room temperature the sample 1 displays a split spectrum, as discussed before. We may now summarize our interpretation of the observed Mössbauer spectra as follows. At any given point of time, half of Mössbauer nuclei find their ‘local’ magnetic field pointing along 0 while the other half will see the local field pointing along [. Both these orientations would of course yield an identical six-finger pattern, because the nucleus as an observer cannot distinguish between 0 and

Memory in Nanomagnets

131

[, provided the local field is static, within the Mössbauer measurement time. That of course is determined by the temperature T and the mean dipolar strength parametrized by Λ. These two quantities determine the rates of relaxation of the dipolar field. Hence, for sample 2, for which the dipolar field is negligible, semblance of a six-finger pattern shows up only at the lowest T when relaxation slows down, whereas for sample 1, the dipolar coupling keeps the relaxation slow within the nuclear time-window, at all temperatures. 5.4. Analysis of Results In the discussion of Mössbauer spectroscopy our focus has been the influence of dipolar interaction on slowing down relaxation. In this section we will turn our attention onto the effect of polydispersity, viz., volume-distribution of the nanoparticles. We will show that such a distribution leads to striking memory effects in low temperature DC magnetization measurements – surprisingly, and somewhat counter intuitively, dipolar interaction suppresses memory effects. The magnetization measurements are carried out in accordance with the following cooling and heating protocol (cf. Fig. 5.18). Starting from room temperature 300K , for our purpose), a small magnetic field of 100 Oe is applied and the magnetization (M) measured. Keeping the field on, the temperature (T) is lowered continuously at a steady rate of 20K/min and M is simultaneously measured upto the temperature Tn (the solid line). At Tn, the field is switched off and the drop of M is monitored for nearly 4 hours (dashed line). Subsequently, the field is switched back on and M(T) versus T is mapped in the cooling regime. Again at Tn-1 the field is switched off and the process of measurement is repeated, until the lowest temperature To is reached. Thus, one obtains field-cooled response and zero-field relaxation of the magnetization. At the end of the cooling cycle, at , , the field is turned on (dashed-dotted line), and M(T) is monitored as the system is heated from T0 through Tn-2, Tn-1, Tn and eventually to , again at the rate of 20K/min, the magnetic field remaining on, throughout. Our results are shown in Fig. 5.19, for samples 1, 2 and 3 (whose attributes are

132

A Paradigm Called Magnetism

Fig. 5.18. Time-temperature protocol.

Fig. 5.19. Magnetization versus temperature data during cooling and heating cycles, for samples 1, 2 and 3.

Memory in Nanomagnets

133

mentioned in Fig. 14 and Table 1). The heating path surprisingly shows wiggles in M(T) at all the T steps Tn-2, Tn-1, Tn where the magnetic field was earlier switched off during cooling, apparently retaining a memory of the temperature steps at which cooling was arrested. More surprising, however, is the fact that memory effects, defined here in terms of overlap of the data during cooling and heating cycles, are the most prominent for sample 3. Recall that for the latter dipolar interaction is negligible. Indeed memory effects are the weakest for the ‘Interacting’ sample 1. Our interpretation is that the observed memory effects are due to polydispersity, most prominent in sample 3, which leads to a superposition of relaxation times, because the volume V occurs in the exponent (cf. Eq. (5.10)). To illustrate this point, we now consider simulation data, for just two sizes (bidispersive), schematically depicted in Fig. 5.20. Recall that the ‘Blocking Temperature’ TB is that temperature at which the experimental timescale of measurement equals the relaxation time, i.e. τÓ τ3 exp :KVk T

PARADIGM CALLED

MAGNETISM

This page intentionally left blank

A

PARADIGM CALLED

MAGNETISM

Sushanta Dattagupta Indian Institute of Science Education & Research Kolkata, India

World Scientific NEW JERSEY . LONDON . SINGAPORE . BEIJING . SHANGHAI . HONG KONG . TAIPEI . CHENNAI

A-PDF Merger DEMO : Purchase from www.A-PDF.com to remove the watermark

Published by World Scientific Publishing Co. Pte. Ltd. 5 Toh Tuck Link, Singapore 596224 USA office: 27 Warren Street, Suite 401-402, Hackensack, NJ 07601 UK office: 57 Shelton Street, Covent Garden, London WC2H 9HE

British Library Cataloguing-in-Publication Data A catalogue record for this book is available from the British Library.

Images on cover design are from http://www.indiaart.com/Online_Exhibitions/online_exhibitions_1.html

A PARADIGM CALLED MAGNETISM Copyright © 2008 by World Scientific Publishing Co. Pte. Ltd. All rights reserved. This book, or parts thereof, may not be reproduced in any form or by any means, electronic or mechanical, including photocopying, recording or any information storage and retrieval system now known or to be invented, without written permission from the Publisher.

For photocopying of material in this volume, please pay a copying fee through the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, USA. In this case permission to photocopy is not required from the publisher.

ISBN-13 978-981-281-386-2 ISBN-10 981-281-386-1

Printed in Singapore.

Benjamin - A Paradigm Called Magnetism.pmd 1

9/2/2008, 5:40 PM

To the cause of integrated Science Education and Research, in India.

This page intentionally left blank

Preface

Magnetism is truly a very old subject. The first reference to a magnetic material, magnetite or the famed loadstone, can be found in Greek literature in astonishingly early times like 800 B.C. Yet the subject remains modern. It appeals to extremely basic issues of physics– magnetism as a material property is a direct result of one of the fundamental forces of nature governed by electromagnetic interactions. At the same time, this property forms the core of technology, influencing power-generation, biomedical applications through, for instance, magnetic resonance imaging, computer industry with the aid of memory devices and chips, just to name a few. Our objective in this volume is not to dwell on the myriad applications of Magnetism but to highlight the rich structure of its theory. It is remarkable to recount how many extraordinary ideas of physics ensue while teaching a course in Magnetism. To mention some: the first instance of velocity-dependent potentials in Mechanics is encountered in treating the Lorentz force on a charged particle in a magnetic field, the first example of the violation of time reversal is stumbled upon when we consider the Zeeman interaction of a spin in an external magnetic field, and so on. Given this background to the wide applicability of the concepts of Magnetism, the purpose of these Lecture Notes is to further amplify how the subject has influenced developments in other diverse areas of Physics and how models used in Magnetism can help to clarify a variety of apparently unrelated phenomena. Magnetism is essentially a quantum mechanical subject. Yet its classical limits such as those described by Heisenberg or Ising-like models have far reaching applications to a

vii

viii

Preface

plethora of topics in phase transitions. Thus, while the ideas of symmetry-breaking and scaling first appeared in Magnetism, they soon pervaded other topics of not just condensed matter physics, but even distant terrains of field theory and high energy physics. Similarly, the concepts of disorder and frustration, embedded in magnetic spin glass systems, are also common to structural glasses. In the domain of nonequilibrium effects too, examples derived from Magnetism help to elucidate the underlying issues of relaxation and dissipation. With the preceding preamble, the Lecture notes are chapter-wise divided as follows. Chapter 1, consisting of three sections, deals with the by-now well-known phenomena which first appeared in the context of Magnetism but have had important bearing in many other subjects. In section 1.1, we discuss the Mermin-Wagner-Berezinskii theorem on symmetry-breaking in the context of the Heisenberg magnet and its implications in φ 4 field theory. The latter forms the backbone of section 1.2 that is devoted to universality and consequent scaling relations which are the underlying concepts in critical point phenomena. In section 1.3 we discuss the issue of multicriticality and point out how the models originally introduced to describe this phenomenon in what are called metamagnets, found their application to tricritical points in 3He - 4He mixtures and even to bicriticality and tetracriticality in an open, nonequilibrium system such as a two-mode ring laser. From chapter 2 onwards, we turn to more recent topics. In chapter 2, we introduce the contemporarily relevant topic of the quantum critical point, again in the context of the Ising model but now in a transverse magnetic field, which finds its realization in rare-earth magnetism. The model helps illustrate the occurrence of quantum phase transitions in a variety of phenomena. The same model allows us to deal with the inter-connected concept of disorder and frustration, which is the subject of chapter 3. Again, the important ideas were first observed in dilute magnets alloyed with metals, called spin glasses. In chapter 4, we move from equilibrium to nonequilibrium statistical mechanics and show how the well-established ideas of spin-lattice and spin-spin relaxations, which are at the heart of magnetic resonance systems, can be further developed to obtain coarse-grained models of phase ordering and pattern formation, seen in many systems as competition between nonlinear interactions and

Preface

ix

nonequilibrium effects. In chapter 5, we discuss important nonequilibrium phenomena seen in an assembly of single-domain nanomagnetic particles. The concomitant relaxation and memory effects are found to be a consequence of the interplay between polydispersity and inter-particle interactions. Similar memory or aging effects are observed in very different systems of relaxor ferroelectrics, shapememory ferroelectric materials and structural glasses. The concepts discussed in chapter 4 in the context of magnetic response and relaxation behaviour find their counterparts in the recently-developed subject of dissipative quantum systems, discussed in detail in chapter 6. Therein we analyze the significance of coherence to decoherence transitions using a magnetic paradigm of Diamagnetism, which is intrinsically a quantum phenomenon, for which the boundary of the container plays a critical role. Thus dissipative diamagnetism is prototypical of decoherence in mesoscopic structures. Our final example is from a large spin quantum system that finds its realization in molecular magnets, and in which mesoscopic quantum tunneling can be seen. The influence of environment-induced dissipation makes this system yet another example of observing coherence to decoherence in quantum to classical crossover phenomena. Acknowledgments I would like to thank the Department of Science and Technology, New Delhi for awarding me the J.C. Bose Fellowship, which enabled me to complete this project. The staff at World Scientific Press in Singapore deserve special praise for being so patient with me despite me missing so many deadlines for manuscript submission. My wife Ranu, daughters Shahana and Sharmishtha, and numerous colleague island friends have been strongly supportive during my challenging days of transition, when this manuscript was being written. I record my warmest gratitude to them. Finally, I thank Manas Roy for help with the figures and Immanuel Alexander for efficient word-processing. Sushanta Dattagupta

This page intentionally left blank

Contents

Preface

vii

1. An Assortment of Well-Established Concepts 1 1.1 Symmetry-Breaking ................................................................................ 1 1.2 Critical Phenomena and Scaling ............................................................. 9 1.3 Multicriticality ...................................................................................... 16 1.4 Multicriticality in an Open System of Two-Mode Lasers .................... 24 2. Quantum Phase Transition: Transverse Ising Model and Other Systems 2.1 Introductory Remarks ........................................................................... 2.2 The Mean Field Theory of TIM ............................................................ 2.3 The Quantum Magnet LiHoF4 .............................................................. 2.4 Quantum Statistical Mechanics ............................................................

29 29 32 36 41

3. Glass Transitions 3.1 Preamble – Magnetic Glass, Quantum Glass, Spin Glass, Proton Glass and Structural Glass ........................................................ 3.2 Magnetic Glass: Li Hox Y1-xF4 ............................................................ 3.3 Quantum Glass: Li Hox Y1-xF4 in a Transverse Field ........................... 3.4 Spin Glasses .......................................................................................... 3.5 Proton Glasses ...................................................................................... 3.6 Structural Glasses .................................................................................

47 47 48 57 59 62 64

4. Relaxation Effects 4.1 Introductory Remarks ........................................................................... 4.2 Single Spin Kinetics in Equilibrium ..................................................... 4.3 Non-Equilibrium Response of a Single Spin ........................................ 4.4 Effects of Interaction on Relaxation .....................................................

69 69 71 78 83

xi

xii

Contents

5. Memory in Nanomagnets 95 5.1 Introduction to the Physics of Single Domain Nanomagnetic Particles ................................................................................................ 95 5.2 Rotational Brownian Motion, the Kramers Problems and Susceptibility ...................................................................................... 106 5.3 Experiments: Stern-Gerlach and Mössbauer Spectroscopy ................ 117 6. Dissipative Quantum Systems 6.1 Introduction ........................................................................................ 6.2 Nonequilibrium Statistical Mechanics ................................................ 6.3 Spin-Boson Hamiltonian .................................................................... 6.4 Dissipative Diamagnetism .................................................................. 6.5 Spin Tunneling and Coherence-Decoherence Phenomenon ...............

139 139 142 148 157 169

References

179

Index

189

Chapter 1

An Assortment of Well-Established Concepts

1.1. Symmetry-Breaking The dynamics of a many body system are determined in terms of a Hamiltonian. The Hamiltonian is characterized by its invariance properties under all transformations that belong to a group, reflecting the underlying symmetries of the system. An extremely rich example of such a system is the one governed by interacting magnetic spins S and described by what is called the Heinsenberg Hamiltonian: H =− J Si ⋅ Sj . (1.1)

∑

The summation is over sites i and j, and is restricted to nearest neighbours, as indicated by the angular brackets < >. The term J is usually referred to as the exchange interaction [1-5]. We may now enlist all the invariance properties of H . The most basic of all these, as is indeed the fundamental attribute of all mechanical systems, is the invariance under time translation. The implication of this invariance is that the total energy is constant, as it must be for a conservative mechanical system. The second invariance property, again shared by most mechanical systems, is the one exhibited under time reversal. As the time t is reversed to −t, each spin operator such as Si has its sign flipped, because S transforms like the orbital angular momentum operator. There is however no overall change in sign for the pair i and j. Time reversal symmetry is fundamental to electromagnetic forces and is broken only due to dissipation, or the presence of an external magnetic field. The third property, which is what we would like to focus onto, 1

2

A Paradigm Called Magnetism

relates to the invariance of H under the simultaneous rotations of all spins through an arbitrary angle about an arbitrary axis. The group of transformations that leaves the Hamiltonian invariant is the symmetry group, denoted by G. If the Heisenberg Hamiltonian does not make a distinction between different orientations, as discussed above, how does it then describe ferromagnetism which is associated with a unique directionality of the magnetization? Recall that the thermodynamic state of a system is governed by the minimum of the Helmholtz free energy F = U – TS, U being the internal energy, S the entropy and T the temperature. For instance, for the magnetic system at hand, the system would choose those spin configurations for which F is minimized. Thus, at high temperatures, the entropy dominates and the maximally disordered state has the highest entropy. This implies that the high temperature equilibrium state is paramagnetic with no average alignment of spin, i.e. the magnetization is zero. Therefore, the paramagnetic phase is invariant under the same group G as its Hamiltonian. On the other hand, at low temperatures, U dominates over TS and the ground state of H is the one in which all the spins are aligned along the same direction. (Note the negative sign in the right hand side of Eq. (1).) This low temperature equilibrium phase is a ferromagnetic one with nonzero average spin <S> = <Si >, independent of the site index i, or equivalently a magnetization, m = µVo–1 <S>, Vo being the volume of a unit cell and µ the magnetic moment per spin. At a critical temperature Tc called the Curie temperature the system undergoes a phase transition from the entropy dominated paramagnetic state to the energy dominated ferromagnetic state. Thus the magnetization m, which is zero in the paramagnetic phase and becomes non-zero in the ferromagnetic phase, is appropriately called the order parameter of the low temperature phase. It is invariant under rotations about an axis parallel to itself but changes under rotations about all axes that are oblique to itself. Therefore, the ordered phase has a lower symmetry than the full symmetry of the group G — it is a broken symmetry phase, as it breaks the symmetry of the Hamiltonian [6, 7]. The important concept of symmetry-breaking transitions, as enumerated above, transcends the subject of Magnetism to many

An Assortment of Well-Established Concepts

3

other areas of Condensed Matter Physics and even to Quantum Field Theory and Particle Physics [8]. Indeed many of the ideas of symmetry and symmetry-breaking transitions in Magnetism, as encapsulated in the Heisenberg or Heisenberg-like models, can be carried over to different fields. We may recall that the most common form of phase transitions in condensed matter physics is encountered in the case of fluids (gases or liquids). A fluid is the highest symmetry phase of matter which is invariant under the Euclidean group of all translations, rotations and reflections. As the external field such as pressure and temperature are varied one sees a series of phase transitions. The most common low temperature phase is a crystalline solid for which the symmetry is lowered from that of the fluid phase. As it turns out the gas-liquid phase transition can be discussed in complete analogy with the magnetic phase transition. While this will be dealt with in Sec. 2 below we want to mention here that in Quantum Field Theory, the idea of symmetrybreaking in a Heisenberg magnet finds its echo in the Lagrangian of n-coupled scalar fields in what is called a φ 4 theory. Although the Lagrangian and hence the equations of motion are invariant under a continuous group of transformations, the ground state, called now the vacuum, is not invariant — the symmetry appears spontaneously broken. This phenomenon is completely akin to a Heisenberg magnet which exhibits spontaneous (i.e. in the absence of an applied magnetic field) magnetization below the Curie temperature. Further, just as in the case of Heisenberg magnets wherein low temperature excitations are described by spin waves (whose quanta are magnons), the consequence of continuous symmetry-breaking in field theory is the appearance of massless excitations called the Goldstone Bosons. Indeed, it is this similarity between Magnetism and Particle Physics which has helped establish the deep relationship between Field Theory and Statistical Mechanics [9-11]. To further underscore this similarity, mentioned in the paragraph above, we may recall the famous Mermin-Wagner-Berezinskii (MWB) theorem [12-14]. It states that a system with a continuous symmetry (such as the Heisenberg model under continuous rotations) cannot have a spontaneously broken symmetry in dimensions less than or equal to two. The theorem is most conveniently proved in a simpler version of the

4

A Paradigm Called Magnetism

Heisenberg model called the XY-model. In the XY-model the longitudinal components (along the Ƶ-axis about which the symmetry of the Heisenberg model is expected to be broken) are assumed suppressed. Thus Eq. (1.1) yields

Hxy = − J

∑ (S S

ix jx

+ Siy Sjy ).

(1.2)

The Hamiltonian in Eq. (2), like the one in Eq. (1.1), is invariant under continuous and arbitrary rotations about the ƶ-axis. In the classical limit Eq. (1.2) may be written as Hxy =− J

∑ cos(θ − θ ) . i

j

(1.3)

Further, in order to obtain the continuous limit of Eq. (1.3) in which the lattice spacing a is arbitrarily small, we can expand the cosine term to yield H=

J 4

∑ γ (θ ij

i

− θj )2 − ξ JN + higher order terms .

(1.4)

ij

In Eq. (1.4), is the number of nearest neighbours (the ‘coordination number’ of the lattice). The restriction on the summations over i and j being over nearest neighbours (indicated by angular brackets in Eq. (1.3)) is removed but is reimposed through the introduction of a matrix γij which is defined as

γij = 1, if i and j are nearest neighbors , = O, otherwise.

(1.5)

Neglecting the constant and the higher order terms in Eq. (1.4) the continuum version is

Hxy =

1 d d xp[∇θ ( x )]2 , 2

∫

where d is the spatial dimensionality and

(1.6)

An Assortment of Well-Established Concepts

p=

ξJ 2d

a2− d .

5

(1.7)

In the XY model the spin vector can point in any direction in the XY-plane, but if the symmetry is broken, one direction is preferred. Assuming that direction to be the X-axis the order parameter is 1 cos Dθe e . Z

1.8

where Z is the partition function and β = (kBT)–1, kB being the Boltzmann constant and T the temperature. Using the ‘Gaussian’ property of Hxy due to which all cumulants of the fluctuations in θ (x) beyond the second order vanish, we find 1

− < cos θ ( x ) > = e 2 .

(1.9)

Furthermore

< θ 2 (x) > = −

∑ q

∂ 1 ∂ βρ q 2 2

ln Z q ,

(1.10)

where # is the wave vector that is Fourier-conjugate to , and 1

2π 2 Zq = βρ q 2

(1.11)

Thus < θ 2 (x) > =

1

∑ βρ q q

2

.

(1.12)

which, in the continuum limit yields 1 ddq 1 1 Λd − 2 < θ 2( x ) > = = , 2βρ (2π ) d q 2 4π 2 ρβ (d − 2)

(1.13)

where Λ is the wave number cut off. Equation (1.13) measures the degree to which the order parameter value is diminished from its zero

6

A Paradigm Called Magnetism

temperature (saturation) value due to classical thermal fluctuations. Evidently as the dimension d approaches the value 2 the fluctuations grow inordinately thereby destroying the order (cf. Eq. (1.9)). This result then proves the celebrated MWB theorem by establishing that fluctuations destroy long range order for a system with continuous symmetry in dimensions less than or equal to two. Physically speaking, the long-wavelength (low q) modes make ‘weighty’ contributions in low dimensions, thermal excitation of which averages out the orientation of the average spin angular momentum. The MWB theorem, first derived in the context of magnetism, has been restated by Coleman in Field Theory. As mentioned earlier, spontaneous symmetry-breaking yields a zero mass Goldstone boson. However, in a two-dimensional space-time it is not possible to construct a massless scalar field operator due to severe infrared (or large wavelength) divergences, as indicated above [15]. While the XY-model discussed above is one kind of anisotropy-limit of the Heisenberg model, a different kind of anisotropy ensues when the transverse components of the spin are suppressed and only the longitudinal components are led to interact. This yields the much studied Ising model the Hamiltonian of which can be written as [16, 17] HIS =− J

∑S S

iz jz

.

(1.14)

Unlike the Heisenberg or the XY-model, the Ising model is evidently endowed with discrete symmetry. This symmetry is classified under a group called Z2 that comprises just two elements: the identity and an element whose square is the identity. This Ising or Z2 symmetry is broken in those phase transitions which have just two ordered states with order parameters simply differing in sign. Naturally there is no MWB theorem in the Ising case, which does exhibit a phase transition in two dimensions. The discrete symmetry has a further consequence that there is no mass-less Goldstone bosons — the spin wave spectrum (depicting the magnon frequency versus the wave number) has a gap at large wavelengths [18].

An Assortment of Well-Established Concepts

7

The Ising model has a special place in history as it provides a vindication of the subject of statistical mechanics through the path breaking work of Onsager who obtained an exact solution for the partition function of the model in two dimensions. Thus the existence of phase transition, a phenomenon that occupies the centre stage in the subject of thermodynamics, could be demonstrated in terms of a microscopic theory namely that of statistical physics [19]. It is interesting to note that although the Ising model was first introduced as a model of a Heisenberg-like magnet in the limit of extreme anisotropy, such as due to crystal field effects, the majority of its applications is in different fields such as gas-liquid transitions or ordering in alloys. Thus, in the context of gas-liquid transitions, it is a common practice to think of a lattice-gas model wherein a lattice is imagined to consist of cells. Each cell can be occupied by a liquid-like particle, or be empty, to depict a gas-like particle. Hence, the basic statistical variable is a binary one, like in the Ising magnet, but now is a ‘pseudo spin’ whose upward projection indicates an occupied cell whereas a downward projection implies a vacant cell. If we define the order parameter as the deviation of the density from its average (of the liquid and gas densities of the corresponding coexisting phases) value, the ordered states of liquid and gas are again characterized by equal and opposite (in sign) order parameters, exactly as in the case of the Ising magnet. Indeed this identification of the order parameter allows us to describe the phenomena near the critical point of a gas-liquid phase transition in complete analogy with a paramagnet-to-ferromagnet transition [17]. This is further linked with the concept of ‘universality’, a subject of Sec. 1.2. As mentioned above, the discrete binary symmetry of the Ising model finds yet another application to materials science. Consider then a solid alloy of just two elements. Each lattice site is imagined to be occupied by either an A or a B-type of atom. Thus the occupation variable is once again an Ising pseudo-spin, but now one encounters two distinct phenomena depending on whether the exchange parameter J in Eq. (1.14) is positive or negative. If J > 0, corresponding to ferromagnetic ordering of the spins in the low-temperature phase, one would see clustering of A-rich (i.e. domains of up spins) and B-rich

8

A Paradigm Called Magnetism

(i.e. domains of down-spins) phases. The order parameter now is naturally a composition variable, depicting the fractional concentration of one or the other (A or B) type of atoms. Although this analogy between what is called the phase ordering of alloys and the Ising ferromagnet is complete as far as static thermal properties are concerned, the kinetics in the two cases are quite different. If one imagines to ‘quench’ (i.e. rapidly cool) a spin disordered paramagnet below its Curie temperature, kinetics of ferromagnetic ordering proceed via preferential flipping of spins from one projection to the other. Thus the order parameter, or the magnetization in the present case, is not conserved. On the other hand, in the alloy case, quenching from the disordered (or paramagnetic-like) phase in which the A and B atoms are randomly distributed, to the ordered phase does not imply transmutation of the chemical identify of atoms but simply an interchange of A and B atoms over neighbouring lattice sites. Therefore, the order parameter is now conserved. This difference between conserved and non-conserved order parameter kinetics leads to distinct morphology of domain growth in the two cases [20]. We now discuss the opposite J < 0 (antiferromagnetic) case. It is clear from Eq. (1.14) that alternate up and down orientations of the spins lower the energy. Correspondingly, the alloy case leads to alternate ordering of the A and B atoms, reflecting the fact that unlike atoms like each other in contrast to the phase-ordering case wherein like atoms prefer to agglomerate together. The J < 0 phase transition is appropriately referred to as the order-disorder transition as can be seen, for example, in beta-brass: a 50-50 admixture of copper and zinc on a BCC lattice. At high temperatures, the Cu and Zn atoms occupy two sub-lattices A and B with equal probability. In the low temperature ordered phase, one set of atoms segregates into the sub-lattice A while the other segregates into the other sub-lattice B. The order parameter: C = CCu,A – CCu,B, where C = CCu,A(CCu,B) is the concentration of Cu atoms in the sub-lattice A(B), is the exact analog of the so-called staggered magnetization of an antiferromagnet. What about kinetics? It is important to note that although kinetic processes involving mutual exchange of A and B atoms on neighbouring sub-lattices conserves the

An Assortment of Well-Established Concepts

9

number of A and B atoms, they do not conserve the sub-lattice order parameter. From the above discussion, it is apparent that a whole range of solidification and ordering phenomena in materials science has derived rich dividends from the analysis of the Ising model in magnetism. In addition to the example of alloys, other transformations that have Ising symmetry are ferroelectric and ferroelastic transitions in which the order parameter is an electric polarization or a spontaneously developed strain, respectively [21]. Further generalization of the Z2 Ising symmetry to Zn symmetry yields yet other interesting phenomena of discrete symmetry changes in condensed matter physics. Thus, the n = 3 case known as the Potts model [22], leads to surface ordering such as krypton absorbed on graphite in which one finds three equivalent ground states commensurate with one Kr atom for every three unit cells of the graphite lattice [23]. We now have a Z3 symmetry-broken transition from a fluid to the commensurate state.

1.2. Critical Phenomena and Scaling Our stated objective in these Lecture Notes has been to employ models and phenomena in Magnetism in order to elucidate developments of similar ideas in other fields. To this end we discuss in this section the extremely important topic of critical phenomena and scaling [24]. Indeed it is not an exaggeration to state that the most profound theoretical advance in physics in the last quarter of the last century has been the successful application of the Renormalization Group (RG) to the critical point phenomena, exploiting and using the ideas of scaling [25-27]. Again it is the second order paramagnetic to ferromagnetic transition at the critical (Curie) point that formed the standard paradigm of critical phenomena, and the Ising and similar models of magnetism became the happy hunting ground for applying RG ideas. We first discuss phase diagrams indicating first order transitions across a twophase co-existing line culminating at an isolated point of second order transition, called the critical point, and then introduce the idea of scaling.

10

A Paradigm Called Magnetism

Fig. 1.1. The magnetic field H, applied in the laboratory along the Ising easy axis, is plotted versus the temperature T. The critical point, indicated by a dot, occurs at H = 0 and T = Tc .

While drawing phase diagrams we follow the Griffiths nomenclature of thermodynamic ‘field’ variables such as temperature, pressure, magnetic field intensity, etc., which remain the same for co-existing phases, and ‘density’ variables such as number density, composition, specific volume, magnetization, etc., which acquire distinct values across the co-existence line [28]. The phase diagrams are drawn in either pure field variables space or mixed field-density variables space. An example of the former for a magnet is shown in Fig. 1.1, in which the magnetic field H is plotted versus the temperature T for an Ising model. The coexistence line (for H = 0) is shown as a solid line for T < Tc and a dashed line for T > Tc ; the black dot is the critical point. Recall from Sec. 1.1 that the symmetry-breaking transition in a magnet occurs spontaneously i.e., in the absence of an external magnetic field. Thus the H = 0 line in Fig. 1.1 plays a special role as it is indeed the co-existence line. Thus, experimentally if one had simply gone on to reduce the temperature one would naturally approach Tc from above along the dashed line. Recalling the Z2 discrete symmetry of a Ising Model (cf. Sec. 1.1) the paramagnetic phase above Tc is a spindisordered phase for which the macroscopic magnetization M is zero, because it is equally likely to find a spin pointing up or down. The

An Assortment of Well-Established Concepts

11

situation is illustrated in Fig. 1.2 which shows the thermodynamic Free Energy F versus M. The curve is schematically a parabola, near M = 0 and the thermodynamically stable state for which F is minimum corresponds to M = 0. As T approaches and becomes very near to Tc the curvature of F near M = 0 becomes vanishingly small (Fig. 1.3) until T is decreased just below Tc when F acquires a double-well structure (Fig. 1.4).

Fig. 1.2. A schematic sketch of the Free Energy F versus the magnetization M, for T Tc .

The two minima of F in Fig. 1.4 are degenerate (i.e. they have the same value of F) corresponding to macroscopic regions in each of which the spins point up or down — the Z2 symmetry is spontaneously broken. The corresponding situation is illustrated in Fig. 1.5 which depictsthe phase diagram in the mixed density-field variables space, i.e., M versus T. The two minima of F in Fig. 1.4 are denoted by M+ and M– (M– = −M+) which are to be read off from the two ends of what is called a tie line, indicated by a solid vertical line in Fig. 1.5. The length of the tie line goes on increasing as the temperature T goes on decreasing until at T = 0 M acquires the saturation value Ms. The entire phenomena, described above, are visualized to occur on the two phase co-existence line (i.e. the solid line in Fig. 1.1). Thus a point on the co-existence line in the pure field space (i.e. in Fig. 1.1), for T < Tc fans out into a line in the mixed space of Fig. 1.5, a feature that is generic and is in conformity with the Gibbs Phase Rule [29].

12

A Paradigm Called Magnetism

Fig. 1.3. A schematic sketch of the Free Energy F versus the magnetization M, for T → Tc .

Fig. 1.4. A schematic sketch of the Free Energy F versus the magnetization M, for T just below Tc .

Having discussed the magnetic phase diagram we now analyse in parallel the phase diagram of a fluid that exhibits a gas-liquid phase transition. Recall from Sec. 1.1 that the gas-liquid transition can be described in terms of a lattice gas model which is directly derived from the Ising model. Thus it is not surprising that the two sets of phase diagrams have striking similarties, as well as important dissimilarities. The field that plays the role of the magnetic intensity in a fluid is the

An Assortment of Well-Established Concepts

13

pressure P and the conjugate variable, analogous to the magnetization M, is the specific volume V. The P-T phase diagram for a fluid, in the pure field variable space and akin to Fig. 1.1, is shown in Fig. 1.6. Again the solid line (but now a curved one) is a two-phase co-existence line on which the gas and the liquid phases co-exist with the same (degenerate) value of the Free Energy (cf., Fig. 1.4). Further, like in the magnet case, one can go continuously around the critical point (Pc, Tc) from the gas phase to the liquid phase and vice-versa. However, for a fluid, we are more accustomed to think in terms of a first order transition in which the specific volume V jumps discontinuously as we cross the co-existence line, accompanied by a latent heat of vaporization unlike in Fig. 1.5 in which the magnetization grows continuously from its value as T is decreased below Tc. This difference between the two cases is amplified below:

Fig. 1.5 The co-existence line (parabola-shaped) depicting the magnetization M versus the temperature T. The vertical lines are tie-lines, defining the values of M for co-existing phases.

In the magnet case the co-existence line corresponds to H = 0, as discussed earlier. This relates to the fundamental symmetry of time reversal invariance, discussed in Sec. 1, which implies that for H = 0 the up and down spin projections are equivalent. There is no such symmetry in the fluid case, hence Pc is non-zero and crossing the two-phase co-existence line (the solid one in Fig. 1.6) along an isobar (i.e. constant pressure) or along an isotherm (i.e. constant temperature) would lead to a discontinuous jump of the specific volume.

14

A Paradigm Called Magnetism

Fig. 1.6. The pressure P versus temperature T for a fluid. The solid line is the gas-liquid co-existence line, the continuation of which (the dashed line) is the critical isochore.

How can then one establish a similarity between the magnet and the fluid cases? The clue is to find the right ‘path’ of approach to the critical point. That particular path turns out to be the critical isochore (the dashed line in Fig. 1.6) along which the density is fixed at its critical value, say nc. Defining then the order parameter of the gas-liquid transition as φ = n – nc, φ remains zero along the dashed line, exactly as in Fig. 1.1 for the magnet case, until one reaches below the ‘critical point’ (Pc, Tc) where from φ grows continuously. The critical point, an isolated point of a second order phase transition as discussed above, is a very special point in the phase diagram of a system. The special nature of the point is related to the fact that certain thermodynamic response functions show divergent behaviour as a function of t = (T – Tc)/Tc, as the temperature T approaches the critical temperature Tc from above. Again, the most widely studied response function turns out to be the one relevant for magnetism and that is the magnetic susceptibility $, which measures the linear response of the magnetization to an applied magnetic field. The function χ diverges as t –γ, as t → 0+ where γ is referred to as a critical exponent. What is further remarkable is not only that a very different property, namely the isothermal compressibility for a different system, i.e. a fluid, is characterized by the same divergent behaviour but that the value of γ is

An Assortment of Well-Established Concepts

15

identical to that of an Ising magnet. This follows from the mapping of the Ising model to a lattice-gas model, as mentioned above. The result is quite astonishing because the two systems under consideration are governed by very different interactions and very distinct physical properties. Indeed it is not just a fluid that shows this commonality of behaviour of its response function near the critical point with a magnet but so do other different physical systems e.g. a ferroelectric or an order-disorder alloy, all of which are said to belong to the so-called Ising universality class. This brings us to the issue of universality which links a whole lot of physically different systems based on the common factors of spatial dimensionality d, the dimension n of the order parameter (=1 for the Ising case) and the range of interactions. The astounding statement of universality is that critical exponents like γ (or β which measures how the order parameter such as the magnetization vanishes continuously as T → Tc) are universal. Thus, to the extent that critical phenomena at a gas-liquid transition in a fluid and a paramagnetferromagnet transition in a magnet are describable in terms of the same Ising model (with Z2 symmetry and short-ranged interactions) in three dimensions, the two very different systems are characterized by the same critical exponents [30]. The universality follows from a very general thermodynamic principle that potentials such as the free energy, are generalized homogeneous functions of temperature and other fields in the vicinity of the critical point. The homogeneity leads to certain scale invariance, the essential idea of which can be summarized as follows. The occurrence of a critical point is in some sense the culmination of the battle between the energy, which dictates order and the entropy, which embodies disorder. Thus, fluctuations, measured by the correlation function of spins at different sites of an Ising magnet, for instance, grow inordinately. Concomitantly the correlation length, that characterizes the distance over which a pair of spins is correlated, diverges at Tc. Thus all other length scales become irrelevant and the only length scale that matters near Tc is the correlation length. This then is the notion of scaling which allows us to estimate how thermodynamic functions and correlations vary with temperature from the dependence of the correlation length on temperature.

16

A Paradigm Called Magnetism

It is this twin concept of universality and scaling that led to the successful application of the renormalization group (RG) by Wilson and others to the critical point phenomena [31]. The RG provides a computational scheme for a class of problems for which fluctuations at multitudes of length scales become important. This scheme was successfully applied by Wilson in the early 1970s to the calculation of critical exponents that led to the theoretical validation of universality. Wilson’s original calculation was in the context of field theories in which one introduces a local order parameter, treated as a continuous classical field and the partition function is written as an integral over all possible values of the local order parameter at all space points. But, the most illuminating treatment of RG theory dates back to 1966 when Kadanoff provided a heuristic explanation of scaling, again in the context of an Ising magnet. This real space treatment called Kadanoff construction, does in fact yield a platform on which to build Wilson’s RG which allows for explicit calculations of critical exponents and scaling relations. The Kadanoff construction can be exactly carried out for the one-dimensional Isuing model and leads to higher dimensional generalization following an approximate method called the Migdal (1975)- Kadanoff (1976) procedure [32]. A natural extension of the procedure, first developed for an Ising model in 1 + ε dimensions, can be nicely extended to the problem of Krypton adsorbed on graphite which, as mentioned at the end of Chapter 1.1, can be described by the Potts model of Z3 symmetry [22].

1.3. Multicriticality The phase diagram for an Ising magnet, discussed in Sec. 1.2 (cf. Fig. 1.1), consists of a single line (for H = 0) along the T-axis. The temperature T is thus the only disordering field. Increase in T causes a first order line of two-phase co-existence to terminate at a point called the critical point which is an isolated point of second order transition. What happens when there is more than one disordering field? In the sense of the Gibbs Phase Rule we will have more “degrees of freedom”, in which case, is it possible that we will have a line of critical points in a

An Assortment of Well-Established Concepts

17

higher dimensional phase diagram? Can we generate special critical points which can be reached by simultaneously fixing two or more disordering fields? The answer is YES, and such critical points, called multi-critical points are the subject of this section. The present analysis is based on what is now called the Blume-Capel model [33, 34]. Imagine a Hamiltonian which describes an Ising-type interaction between nearest neighbours which however are now spin-1 ions in a lattice that are subject also to a crystal field ∆:

H=−J

∑S S

ij jz

+∆

2 iz ,

∑S

∆>0

(1.15)

i

Clearly, the crystal field terms would simply be a constant for the ordinary spin half Ising model discussed hitherto. Here Si = ±1 or 0 and one now can consider two disordering fields T and ∆ shown in Fig. 1.7 For ∆ = 0, we are back to our earlier Ising case, in which we have the usual ferromagnetic to paramagnetic transition but now occurring along the ordinate (in constrast to Fig. 1.1). For small enough ∆ the single ion energy levels Si = ±1 lie not much higher than Si = 0 singlet and so the exchange interaction remains operative. Under this condition, mean field calculations suggest that the paramagnetic-ferromagnetic transition continues to be of second order as in the ordinary Ising model. As ∆ is increased one sees a line of critical points (the solid line in Fig. 1.7), until beyond a critical value ∆c, the transition changes into a first order one and the cross-over occurs at what is called a tricritical point [35]. As ∆ is increased still further, the transition temperature decreases and goes to zero. This is so because, for a large value of ∆ the Si = ±1 levels become inaccessible and hence the exchange interaction becomes inoperative. The following features about the various terms in the Hamiltonian in Eq. (1.15) are worth noting in our understanding of tri-critical behaviour. First, one has the usual magnetic order M = <Si > which characterizes the ferromagnetic to paramagnetic transition. In addition, one has, for this spin-1 system, a quadrupolar order parameter Q = <Si2 >. Note that the field ∆ which is conjugate to Q plays the same role as H does with respect to M. Further, the order parameters M and Q are not totally

18

A Paradigm Called Magnetism

Fig. 1.7. Phase diagram in the T – ∆ plane. For ∆ < ∆c, one has a second order transition from the para-to-ferro-magnetic phase. For ∆ > ∆c, the transition changes over into first order (dashed line).

independent of one another. For example, it is not possible to have a stable state in which M = 1 and Q = 0, since M = 1 requires that all the spins have Si = 1 which in turns leads to Q = 1. The two-order parameters are therefore kinematically coupled in the sense that even in the absence of interactions, there are constraints on the values which can be taken on by the two together. It is the competition between the two kinematically coupled order parameters which is eventually responsible for the occurrence of the tricritical point. The exchange term in Eq. (1.15) gives a lower energy for M = 1, while the crystal field term favours Q = 0. These two values are incompatible, however. The increase in ∆ ultimately makes it more favourable energetically to have Q = 0 (and hence M = 0) than M = 1. The meaning of the various phases, that are expected to occur in relation to Fig. 1.7, become clearer if one considers an applied magnetic field H in addition to the crystal field and Ising terms in Eq. (1.15). The Hamiltonian now becomes

H=−J

∑S S

iz jz

+∆

∑S

2 iz

i

−H

∑S

iz

i

.

(1.16)

An Assortment of Well-Established Concepts

19

The corresponding phase diagram, in the space of three field variables (in the sense of Sec. 1.2): T, ∆ and H, is shown in Fig. 1.8. The two-dimensional phase diagram shown in Fig. 1.7 is a projection of the three-dimensional diagram of Fig. 1.8 onto the H = 0, (T – ∆) plane. One now has a first order co-existence surface A in the H = 0 plane, on which the order parameter M assumes nonzero values with opposite signs depending on whether H → 0 from positive or negative directions, exactly as in Fig. 1.7, for T < Tc. As T increases, keeping ∆ ‘small’ the surface A terminates in a line of critical points (the bold solid line on the H = 0 plane in Fig. 1.7). However, for T < T * and ∆ > ∆*, this line of critical points terminates in the two-phase co-existence line D, which is a line of first order transitions, shown as a dashed-dotted line in Fig. 1.8. Looking at Fig. 1.8 one notes that A is connected along the line D to two first order (co-existence) surfaces B and B′ extending symmetrically into the regions H > 0 and H < 0, respectively. The surfaces B and B′ themselves terminate with increasing temperature in lines (bold solid ones) of critical points. These two critical lines (for H ≠ 0) fan out symmetrically from the H = 0 plane and join the critical line (for H = 0) at the tricritical point (the black dot). Thus, the tricritical point may be regarded either as the termination of a line (D) of triple (or three-phase co-existence) points, or equivalently, as the confluence of three lines of critical point. In fact, it is the latter feature which prompted Griffiths to name the special point a tricritical point [35]. We will return to further discussion of the phase diagram in Fig. 1.8 in the context of a very different system, viz. a He3 – He4 mixture. A model of the kind described by Eq. (1.15) has been used by Blume to explain first-order magnetic phase changes in UO2 [33]. It was found that depending on the ratio of the crystal field splitting ∆ to the molecular-field splitting (appropriate to the exchange term in Eq. (1.15)), one obtains either a paramagnetic state, a first order phase change (indicated by the dashed line in Fig. 1.7), or a second order transition (shown as the solid line in Fig. 1.7). The confluence of the first order line and the second order line, viz. the black dot in Fig. 1.7, is a tricritical point, as discussed above. While the tricritical phenomenon in UO2 takes place in the absence of an external magnetic field, first-order phase transitions are known to occur in magnets to which an external magnetic

20

A Paradigm Called Magnetism

field is applied. Such systems are known as meta-magnets. A case in point is the system of FeCl2 which belongs to a class of meta-magnets that exhibit a tricritical point [36]. The mechanism is discussed below.

Fig. 1.8. Phase diagram for an Ising magnet in the presence of a crystal field ∆ and a magnetic field H. There are three surfaces of first order transitions A, B, and B′, which meet at the tricritical point that may be viewed also as the meeting point of three lines (solid) of second order phase transitions.

In FeCl2, Fe ions are placed on stacks of parallel triangular lattices separated by Cl ions, as shown in Fig. 1.9. Each Fe ion is surrounded by a cage of six Cl ions. The iron is in the valence state of Fe2+ and carries an effective spin of one. The sign of the exchange interaction within a layer is positive, favouring ferromagnetism whereas that between layers is negative yielding anti-ferromagnetism. Further, the spins are preferentially aligned perpendicular to the layers because of lattice anisotropy. Thus, in the fully ordered state, the spins in a given plane are parallel, but they alternate in direction from layer to layer, thereby yielding a two-sub-lattice anti-ferro-magnetic order. When an external magnetic field is applied normal to the layers, the sub-lattice magnetization which is conducive to the applied field will show enhancement, whereas the neighbouring sub-lattice magnetization will undergo a decrease. Thus, there occur both a uniform magnetization and

An Assortment of Well-Established Concepts

21

Fig. 1.9. Crystal structure of FeCL2.

a sub-lattice magnetization. Again, we have a situation with two competing order parameters, like in the example discussed in the beginning of this section. When the applied field is large enough to polarize all the spins, anti-ferro-magnetic order will be destroyed. The experimental phase diagram for FeCl2, for which the uniform magnetization m is plotted along the ordinate and the temperature T is plotted along the abscissa, is shown in Fig. 1.10. When T is large and the uniform magnetization is sufficiently small we are in the anti-ferromagnetic (AF) phase. Keeping T fixed on the high temperature side and enhancing m, as can be achieved by increasing the strength of the applied magnetic field, one crosses into the paramagnetic (PARA) phase, as argued above. The line of demarcation is a line of critical points i.e. a line of second order phase transition. Below a certain temperature indicated by a black dot and labeled by Ttr, we have phase separation, meaning thereby that two phases, one with ‘large’ uniform magnetization and the other with small uniform magnetization (and concomitantly, a

22

A Paradigm Called Magnetism

‘large’ staggered magnetization), co-exist. The point Ttr is the tricritical point.

Fig. 1.10. Schematic phase diagram for the metamagnet FeCl2.

It may be noted that the phase diagram in Fig. 1.10 is in the mixed density-field variables space, in accordance with the nomenclature introduced in Sec. 1.2. Thus the portion of the diagram to the left of T * looks qualitatively like the magnetization versus temperature diagram of an ordinary ferro-magnet. Had we drawn the phase diagram in the field variables space by replacing the magnetization by its conjugate magnetic field the two-phase co-existence region would have shrunk to a first order line, meeting the second-order line at the tricritical point, as in Fig. 1.7. A very similar phenomenon of tricritical points is found in a completely different system of a binary mixture of He3 and He4 in which He4 can occur in two different phases: normal and suverfluid, the two phases being related by a symmetry operation. Indeed a slight modification of the Hamiltonian as employed in Eq. (1.16) for the metamagnet FeCl2 goes under the name of the Blume-Emergy-Griffiths (BEG) model that was used for describing the tricritical point in He3 – He4 mixtures [37]:

23

An Assortment of Well-Established Concepts

H = − J ∑ Siz S jz − K ∑ ( Siz )2 ( S jz )2 + ∆ ∑ Siz 2 − H ∑ Siz . (1.17) < ij >

< ij >

i

i

Under saturated vapour pressure it is observed that the superfluid %-transition temperature decreases with increasing mole fraction x of He3, and below a temperature & ' 0.87* corresponding to 0.67, a first order phase separation takes place (Fig. 1.11).

Fig. 1.11. Phase diagram (schematic) for /5 6 0 /5 7 mixtures. The two-fluid coexistence curve is labeled D, the dashed curve is the line of the lambda transitions and the dot indicates the tricritical point.

The corresponding phase diagram in the space of field variables is the same as in the case of the metamagnet FeCl2 (Fig. 1.8) in which ∆ may be interpreted as the themodynamic field conjugate to x, i.e., ∆ is the difference in chemical potentials of He3 and He4, and H is a fictitious field conjugate to the superfluid order parameter .. The first order coexistence surface A in the / 0 plane extends to ∆ 01 (pure He4). On A, . assumes nonzero values with opposite signs, as described earlier following Eq. (1.16). Thus . is the analog of the magnetization M, the order parameter in the magnetic case. The BEG model has a built-in time-reversal symmetry (in the absence of H) with the consequence that odd terms in the spin operator 234 , for instance, are absent. The most general spin-one model however, which subsumes the BEG model, Eq. (1.17), and the Hamiltonian for the metamagnet, Eq. (1.16), does not have to obey this symmetry, and is

24

A Paradigm Called Magnetism

therefore, applicable to a ternary liquid mixture. The corresponding Hamiltonian can be written as [38]:

08 9 234 2;4 0 * 9 234 = 2;4 = 0 > 9 234 = 2;4 :3;

is independent of the site index j. Therefore H i ≡ H = J (0) < S z >, where z

J (0) = Z J ij .

(2.4)

Hi = −( HS zi + ΓS xi ).

(2.5)

j =1

Hence, Eq. (2.2) yields

The partition function is given by

ƕ( %012 3 4 56Ɩ 7 869 :,

2.6

where < = %& . Because S z takes only two discrete values +1 and −1 we can use properties of 2x2 matrices to decompose the exponential operator in Eq. (2.6), in order to simplify ƕ( as

Z i = 2 cos ℏ (βh ),

(2.7)

independent of i and where

h=

H 2 + Γ2 .

(2.8)

Thus

< S z >=

1 Tr [ S zβ ( HJ z + ( ΓS x ) ], 2 cosh( β h )

(2.9)

which yields

< sz >=

H tanh( β h). h

(2.10)

34

A Paradigm Called Magnetism

Similarly,

< S x >=

Γ tanh( β h). h

(2.11)

Denoting the LHS of Eqs. (2.10) and (2.11) as the components of the magnetization mz and mx respectively, we obtain the transcendental equations:

mz =

mx =

J (o ) m z

tanh( β ( J (o ) mz ) 2 + Γ 2 ),

(2.12)

Γ tanh β ( β ( J (o)mz ) 2 + Γ 2 ). ( J (o ) mz ) 2 + Γ 2

(2.13)

2

( J (o) mz ) + Γ

2

The above equations yield self-consistent relations for the two relevant magnetization components. Note that the order parameter mz vanishes when either Γ or T goes to infinity. This confirms our earlier physical argument that Γ acts as a disordering field. We may now discuss the phase diagram predicted by Eqs. (2.12) and (2.13) by designating the order parameter mz as ψ and defining the critical temperature for the pure >. . ? 0 Ising model as

Tco =

J (o ) kB

(2.14)

Equation (2.12) then yields (for the solution corresponding to ψ ≠ o )

o 2 T 1= tanh c ψ + Γ 2 , T Tco ψ / T )2 + Γ 2 Tco / T

(2.15)

where Γ = β Γ. At the phase boundary, ψ = o, thus leading to

$

TBC tanh?I$ , 8DB

2.16

Quantum Phase Transition: Transverse Ising Model and Other Systems

35

which is equivalent to

Γ Γ = tanh . J (o) K BTc

(2.17)

The corresponding phase diagram is shown in Fig. 2.1 demarcating the following three regimes:

Fig. 2.1

Region I, where Γ is large, and T is small – quantum effects are dominant here. Region II, where Γ is small – classical effects are dominant and the TIM is analogous to the usual Ising model. Region III, where both Γ and T are moderate. We next analyze the static susceptibility in region III, by adding a small aligning field ∆H along the Ƶ-axis. In that case, Eq. (2.15) can be rewritten as

36

A Paradigm Called Magnetism

ψ=

β∆H + Tco

ψ

ψ tanh ( β∆H + Tco T ) 2 + Γ 2 . ψ ( β∆H + Tco T ) 2 + Γ 2 T

(2.18) Linearzing in ψ and ∆H leads to

Tc0 tanh tan ℏΓ ψ 1 − = β∆H , 2 T Γ Γ

(2.19)

yielding for the susceptibility −1

ψ tan Γ tan Γ χ= = T − Tc0 . ∆H kBΓ Γ

(2.20)

Thus, χ diverges at the critical temperature Tc given by Eq. (2.16) with a mean field critical exponent K 1. Alternatively, χ can be rewritten as

χ = tanh Γ(Γ − KBTco tanh Γ)−1 ,

(2.21)

which again shows a divergence at the critical value of the transverse field Γ = Γ c given by Eq. (2.16) with the same exponent K 1.

2.3. The Quantum Magnet LiHoF4 The system LiHoF4 belongs to a class of compounds LiRF4 , where R is a rare earth element (Fig. 2.2). Although the rare earth elements of Ho 3 + in LiHoF4 are coupled by dipole-dipole interaction, only the lowest doublet of the 17 crystal-field-split states is appreciably populated at low temperatures (T < 2 K ) because of a large crystal field. Further, the sign of the crystal field is negative; hence the lowest doublet corresponds to the highest spin states. Consequently, the off-diagonal terms of the dipolar interaction are effectively “quenched” leading to the so-called “truncated dipolar Hamiltonian” [45]. The latter is of the Ising

Quantum Phase Transition: Transverse Ising Model and Other Systems

37

Fig. 2.2. The Crystal structure of LiHoF4.

type, yielding an Ising coupling between spins projected along the crystallographic c-axis, with the interaction J ij of the form:

1 − 3cos 2 θ ij J ij = J , rij3

(2.22)

where θ ij is the angle between the Ising axis (i.e. the c-axis of the crystal) and the position vector connecting the spins. As seen in −3 Eq. (2.22), J ij is very long-ranged because of its rij dependence on the inter-spin distance rij . This indicates that a mean-field treatment will be in order for such a system. However, the angular dependence [1 − 3cos2 (θij )] allows for J ij to change sign, implying that the interaction switches from ferromagnetic ( J ij > o) to antiferromagnetic While this ( J ij < 0) for intermediate angles (55 ≤ θij ≤ 125 ) . occurrence of competing interactions may raise doubts about the uniqueness of the ground state, a classic analysis by Luttinger and Tisza [46] demonstrates that the ground state is indeed that of a dipolar ferromagnet for the b.c.c structure of LiHoF4 . The experimentally measured critical temperature for the paramagnetic – ferromagnetic transition turns out to be Tc = 1.53K . Having arrived at a situation in which one has an Ising model as an approximate low-temperature description of the dipolar-coupled system,

38

A Paradigm Called Magnetism

the question arises: How does one realize a TIM? In the experiment of Bitko et al. [47], a small magnetic field H t transverse to the c-axis is applied in the laboratory which causes admixture of the two eigenstates of the crystal-field-split doublet (See Fig. 2.3), yielding (in perturbation theory) a spin Hamiltonian that is proportional to S x , with a prefactor Γ∞H t2 . Thus, single crystals of LiHoF4 provide a clean model system in which high-precision, controlled investigation of quantum critical phenomena can be performed. In one other aspect, LiHoF4 is unusual in that the observed magnetic behavior is quantitatively described by mean-field theory, discussed in Sec. 2.2 [48]. The fact that the quantum critical behavior in d = 3 is mean field-like is not surprising as it is known that the d-dimensional quantum phase transition (at T = 0) for the TIM is equivalent to the ( d + 1) dimensional thermal phase transition for the ordinary Ising model [49, 50]. The mean field nature of the thermal phase transition observed in LiHoF4 is also not surprising as renormalization group (RG) theory shows that, for a dipolar-coupled Ising system, the marginal dimensionality is L$ 3, barring logarithmic corrections for critical exponents. [51]. (Recall that we expect mean field behavior for d > d c .) We now bring-in one additional attribute of the LiHoF4 system that is crucial for a satisfactory understanding of the experimentally observed phase diagram, especially at low temperatures. The ionic spin of Ho3+ element has a non-negligible hyperfine interaction with the nuclear spin of Ho in which the coupling constant is of the order of 0.039K. Because the large crystal field ‘quenches’ the off-diagonal terms of the spin operator of Ho3+ (with the crystallographic c-axis as the direction of quantization), as mentioned before, the hyperfine interaction is also axial [48]. Incorporation of this interaction generalizes the Hamiltonian in Eq. (2.1) to: N

N

H = −∑ J ij Siz S jz − Γ∑ Six − a∑ Iiz Siz ,

i =1

i =1

(2.23)

Quantum Phase Transition: Transverse Ising Model and Other Systems

39

where ‘a’ is the hyperfine coupling constant and I iz is the nuclear spin of the ith Holmium nucleus. Correspondingly the single site mean field Hamiltonian in Eq. (2.2) has to be generalized to:

Hi = −[( H i + aI zi ) S zi + ΓS xi ].

(2.24)

With the Hamiltonian in Eq. (2.24) we now proceed to evaluate the phase diagram [52]. In accordance with our earlier analysis the partition function for a single site in the mean field approximation can be written as

ƕ 34 57MNO 6P7869 :,

2.25

independent of i and in which the trace is over the ionic as well as the nuclear spin eigenstates of Ho. Labeling the 8 nuclear eigenstates by |S , we have TƖ |S S|S where M assumes values – 7/2, -5/2, ………5/2, 7/2. Thus +7/2

Z=

∑

2 cosh β h( M ),

(2.26)

( H + aM ) 2 + Γ 2 .

(2.27)

M =−7/2

where h(M ) =

Proceeding as before, Eq. (2.12) for the order parameter can be written as

∑[ mz =

M

aM + J (o ) mz ]Sinh ( β h ( M )) h( M ) . ∑ cosh( β h( M ))

(2.28)

M

The phase boundary shown in Fig. 2.3 is estimated from a numerical solution of Eq. (2.28). The solid curve drawn through the dots is merely a guide to the eyes. The dashed line is the phase boundary in the absence of hyperfine interaction, as shown also in Fig. 2.1. The inset shows the experimentally obtained phase boundary of Bitko et al. from susceptibility measurements (filled circles) and the calculated mean-field phase boundary (solid line) in the presence of hyperfine coupling

40

A Paradigm Called Magnetism

from an 136 x 136 eigenfunction space of the full Hamiltonian (nuclear spin = 7/2, ionic spin = 8) [48]. The dashed line in the inset is the result of computation in the absence of hyperfine interactions. The deviation of the phase boundary from the dashed line for high values of the transverse field Γ can be understood from the following physical considerations. For small Γ the local mean-field is dominated by the effective Ising interaction proportional to the magnetization along the c-axis. However, as Γ increases, the magnetization along the c-axis goes on decreasing (because of the gradual loss of the quantization axis) leading to the situation in which the local field is totally dominated by the hyperfine coupling alone. Because it is the competition between the local field and the transverse field that determines the phase boundary between the ferromagnetic and paramagnetic phases, the ferromagnetic order persists for a larger values of the transverse field, especially at low temperatures, since the hyperfine field takes over the role of the local mean field. This analysis is in conformity with the experimental observation of Bitko et al. in that there is an upward tilt in the phase boundary for temperatures lower than 0.6K [48].

Fig. 2.3. The crystal field splitting in LiHoF4, indicating that at ultra low temperatures, one has an effective 2-state model.

Quantum Phase Transition: Transverse Ising Model and Other Systems

41

2.4. Quantum Statistical Mechanics With the preceding background to quantum phase transition (QPT) in the context of an example borrowed from Magnetism we turn now to the general statistical mechanics discussion on why a QPT is so different from its classical counterparts. Note that the main issue in evaluating the partition function in statistical mechanics concerns the diagonalization of the Hamiltonian. Once this is done one can choose to work in a representation in which the Hamiltonian is diagonal and then compute the trace of the density operator %41 merely in terms of the eigenvalues of H , for completing the calculation of the partition function. The reason this task is difficult in general in a quantum problem is evident from the example of the transverse Ising model; the Ising term is diagonal in the representation of the spin operator , , while the transverse term is diagonal in the representation of the spin operator S x ! Thus there is no definite axis of quantization and hence, the task of diagonalization is humongous, barring the special case of one dimension, or finite systems. This problem is of course peculiar to quantum mechanics because in classical statistical mechanics the kinetic energy and potential energy terms (which add up to the Hamiltonian H ) can be dealt with separately. The term in the partition function involving the kinetic energy yields a Gaussian integral over the momentum variable that leads to a simple temperature – dependent prefactor and all the many body effects are subsumed in the potential energy term. Not that it always leads to a happy situation as far as an exact calculation of the partition function is concerned, as we very well know from the examples of the ordinary Ising model in three dimensions, or interacting classical liquids, etc., but the first battle is won, viz., the kinetic and potential energy terms can be disentangled. Indeed it is this attempt towards disentanglement that yields the basis of the Feynman’s path integral formulation of the partition function, as discussed below [53]. The partition function in the canonical ensemble can be written in terms of a summation over a complete set of states:

U < ) WX %41 XW . V

2.29

42

A Paradigm Called Magnetism

Note that the density operator %41 is identical to the timedevelopment operator e −iHτ /ℏ , if the time τ is considered to be imaginary: τ = −it β . Thus Z is the sum of transition amplitudes for the system to start from some state f > and return to the same state f > after a time interval − iℏ β . The total time interval, which is fixed by temperature, will naturally be infinitely long (along the imaginary axis) at 0! The idea of Feynman is to break up the net transition amplitude between the states of a system into a series of transition amplitudes over intermediate states and summing over all possible paths between the two states. The path in question is defined by specifying the state of the system as a sequence of finely spaced intermediate time steps. One may formally write

e − β H = [e

1 − δτ H N ℏ

] ,

(2.30)

where δτ is a small time interval given by δτ = ℏ where E is taken to E be larger than the highest energy scale in the problem, and N is an integer chosen such that N δτ = ℏ β . We now use the Trotter identify [54]: d c

d

[\ ]^ _>` a a a ,

2.31

ab∞

where [\ and ]^ are two bounded quantum operators. Writing H as H = Τ + V , where T is the kinetic energy operator and V the potential energy operator, the kinetic and potential energy terms can be disentangled in the limit e b 0. Hence the idea of employing a small time interval δτ is to enable the use of classical-like methods by ignoring the non-commulativity of T and V over the small time segment δτ ! Using a succession of closure property the partition function may be rewritten as

U < ) )

&

V Vj Vk …Vm

x < f1e

1 − δτ H ℏ

W f %ghi5 f W&

| f 2 >< f 2 | .... | f N >< f N | e

1 − δτ H ℏ

| f >.

(2.32)

Quantum Phase Transition: Transverse Ising Model and Other Systems

43

j

Note that a typical matrix element such as W& n %ghi5 n Wo signifies an amplitude of transition (in imaginarily time >e from the state |W& to the state |Wo . This is reminiscent of a transfer matrix that connects one site to another in classical statistical mechanics of the Ising model, for instance [17]. Therefore, in the present case, the imaginary time may be thought of as an extra spatial dimension. This indeed is the reason why the statistical mechanics of a d-dimensional quantum system can be viewed equivalent to a ( d + 1) − dimensional classical system, except that the extra dimension is finite in extent, going to infinity only at T = 0 . The underlying idea can be illustrated in terms of the following physical example.

Fig. 2.4. Josephson junctions (crosses) demarcating superconducting grains.

Consider a one-dimensional array of Josephson junctions shown schematically in Fig. 2.4 [44]. The crosses indicate junctions between superconducting grains. Over each grain the superconducting state is characterized by a condensate wave function. Josephson tunneling of cooper pairs from one grain to another occurs across the junctions. The order parameter at hand is the condensate wave junction itself which iθ for the j th grain can be written as ψ j = a j e j . As it turns out it is the fluctuations of the phase angle θ j that are relevant while those of the amplitude a j can be ignored. Because tunneling involves overlap of the wave function between grains, the corresponding interaction Hamiltonian is proportional to the projection operator |p+ p+7& | between the j th and its neighboring ( j + 1) th grains. If coherence of the wave function is maintained, tunneling is facilitated and the system (i.e. the one-dimensional array) is super-conducting. This process however is

44

A Paradigm Called Magnetism

counter balanced by the energy required to transport an excess cooper pair onto a grain, i.e. the coulomb repulsions between pairs. If this energy is large, especially for small grains, the Cooper pairs will be blockaded and the system becomes an insulator. It is this superconductor-insulator transition which is the underlying QPT in the present instance. Given this background the Hamiltonian for the Josephson junction array can be written as:

1 o 1 )q^+ ) r+ stu^+ u^+7& , 2 +

+

2.33

where the hat over a dynamical variable the phase angle signifies its operator nature, E j is the Josephson coupling strength, C is the intra-

grain capacitance and q^+ is the ‘voltage operator’ for the j th grain. Λ

Because q^+ is conjugate to the dynamical variable θ it has a differential j

operator form (analogous to the co-ordinate representation of the momentum operator in quantum mechanics): Λ 2e ∂ . V = −i j C ∂θ j

(2.34)

(Note that the extra factor of 2 in front of e accounts for the total electric charge of a Cooper pair). Substituting Eq. (2.34) in Eq. (2.33) the Hamiltonian can be rewritten as

H = − Ec ∑ j

Λ Λ ∂2 − ∑ E j cos(θ − θ ), 2 j j −1 ∂θ j j

(2.35)

where

Ec =

2e 2 . C

(2.36)

The first term in Eq. (2.35) is analogous to the kinetic energy of a rotor where Ec−1 is like the moment of inertia.

Quantum Phase Transition: Transverse Ising Model and Other Systems

45

At this stage it is possible to draw an analogy between the Hamiltonian in Eq. (2.35) and that of the TIM (cf., Eq. (2.1)). The Josephson energy is akin to the pure Ising coupling in that each interaction favors ‘order’ be it in the form of preserving the phase coherence of the condensate wave function or ferromagnetism respectively. The charging energy, proportional to E c is like the transverse term Γ of TIM that has the effect of disrupting order by effecting quantum transitions between the eigenstates of the angle Λ

operator θ (or the spin operator S jz , in the TIM case). Understandably j

then, the disordering field or the control parameter for the quantum phase transition in the Josephson junction array is expected to be proportional to the ratio of E c and E j . (For a precise relation, see below). When this ratio exceeds a certain critical value the system transits from the superconducting to the insulating phase. As discussed before in the context of the expression for the partition function (Eq. 2.32), each transition amplitude < f1 | e

1 − δτ H ℏ

| f2 >, which

is a statistical weight of a space time path, is the Boltzmann weight of the classical configuration for an equivalent 2d-classical model, in which the extra dimension is along the imaginary time axis. The latter turns out to be the 2-dimensional classical XY-model, the Hamiltonian of which has already been introduced in Eq. (1.3). The angles θ i are now to be interpreted as those of planar spins that lie on a two-dimensional square lattice. It turns out that the coupling constant J is proportional to E J / EC . The inverse of J is then a ‘fake’ temperature for the model, the increase of which causes the coherent ordering of the phases (for the original model) to disappear. On the other hand, a large value of J makes it unlikely that the angles θ i and θ j will differ significantly, even when the sites i and j are far apart (in space and/or time), yielding a superconducting phase. We should emphasize that this equivalence between the one-dimensional Josephson junction array and the twodimensional classical XY-model is only in the sense of universality near the corresponding critical points (cf., Chapter I). Other than that

46

A Paradigm Called Magnetism

however the underlying proof of equivalence goes over to d-dimensional arrays and ( d + 1) − dimensional classical XY models. This is a very useful result in that numerical methods such as Monte Carlo techniques can be applied to study the critical behaviour of d-dimensional quantum models. In conclusion, we note that all the basic ideas of quantum phase transitions and the concomitant quantum critical points have not only a historical connotation to Magnetism but are also most easily understood within the context of a magnetic model eg. the transverse Ising model. Further details of zero temperature (T = 0) dynamic scaling, finite-size scaling for T ≠ 0, and Quantum Hall Effect as a prototypical experimental system of QPT can be found in the eminently readable review article of Sondhi et al. [44].

Chapter 3

Glass Transitions 3.1. Preamble Magnetic Glass, Quantum Glass, Spin Glass, Proton Glass and Structural Glass One of the enigmatic unresolved issues of the contemporary materials physics is the glass transition. The problem is simply stated in the context of an ordinary, monatomic liquid. When the latter is cooled very slowly, i.e. adiabatically such that at every stage of the cooling process the liquid is in thermal equilibrium with the heat bath in which it is embedded, it usually freezes into a crystalline solid at a temperature TF. However, when the liquid is rapidly cooled, i.e. supercooled, it solidifies into a disordered amorphous structure called glass, which has no translational or orientational symmetry unlike a crystal. The transition temperature TG ( TB leads to paramagnetic response which is Curie like (T −1 ) whereas T < TB blocks the magnetization. Polydispersity (i.e., size distribution) will of course cause a broadening of the hump. 5.3. Experiments: Stern–Gerlach and Mössbauer Spectroscopy With the introductory background to the phenomenology of singledomain nano-magnetic particles and the underlying relaxation theory we turn our attention in this section to experimental measurement of the relevant properties. The parameters of interest which can be extracted from experiments are: a) b) c) d)

size or volume V of the particles; the magnetic moment per unit volume µ; the anisotropy energy K, which provides the barrier to relaxation; polydispersity, viz., the distribution function that characterizes the size-distribution, if there is any; e) and interparticle interaction, the most commonly encountered one being the dipolar one. We have so far ignored (e) and considered only independent, noninteracting magnetic particles, and the only measurement techniques we have touched upon in passing are the magnetization and the susceptibility. In what follows, we shall examine a variant of the celebrated Stern-Gerlach setup that has been recently used to study relaxation of nanomagnetic particles, especially magnetic clusters [117].

118

A Paradigm Called Magnetism

Magnetic Clusters in a Stern-Gerlach Setup The experimental configuration is shown in Fig. 5.9. The only difference with the historic experiment is what are jettisoned from the oven are not singly charged Ag ions but single-domain clusters of Co, Gd, etc. For a cluster whose magnetization µV is polarized along the direction z of the inhomogeneous magnetic field one would have expected in the old measurement that the deflection d on the detector screen, measured from z = 0 , would be given by

d=

µV M

B ′ (o )

LD L (1 + ), 2 v 2D

5.63

where m is the mass of the particle, is the gradient of the magnetic field B(z) at z = 0, v is the (constant) speed with which the jet emanates from the oven in the forward (i.e. normal to z-axis) direction and the Length L and D are defined in Fig. 5.9.

S

Fig. 5.9. Stern-Gerlach Setup.

The first contribution within the round brackets in Eq. (5.63) comes from ballistic motion outside the magnet while the second term arises from the accelerated motion within the magnet. Though Eq. (5.63) is wrong in the present discussion because of rotational relaxation of the cluster magnetization within the magnetic pole-pieces region, as will be shown below, it allows for the introduction of an important parameter GS that defines the experimental time-window for the setup at hand:

119

Memory in Nanomagnets

τE ≡

5.64

L . v

The reason Eq. (5.63) is wrong is that the velocity v¡ of the cluster, derived from the acceleration gained in the z-direction in view of the force exerted by the inhomogeneous magnet on the magnetic moment of the cluster, is now a stochastic process, given by P

v¡ ¢ cos , 3

(*

5.65

where ¢ is a constant parameter of the experiment: ¢ ¤ ¥ and θ (t ) is the angle between the magnetic field (i.e. z-axis) and the magnetization vector of the particle. For reasons discussed in detail in Sec. 5.2 the relaxational dynamics of cos θ (t ) may be described in terms of the Fokker-Planck equation (5.25). We would like to dispose of one red herring in order to facilitate comparison with experimental data. Note that the initial conditions chosen on v¡ is that it is zero at time t = 0 , implying that the molecular jet is unidirectional. However, while this is predominantly so, there is a small residual fluctuation in the velocity in the z-direction due to the temperature Ts of the source i.e. the oven. That is, over and above the very large speed of the jet along the dashed line in Fig. 5.9, there is an envelope of velocity distribution governed by a Maxwellian at temperature Ts, thus P

where

v¡ ∆v¡ & ¢ cos , 3

< (∆v z ) 2 >=

k BTs . m

5.66 5.67

120

A Paradigm Called Magnetism

Fig. 5.10. Line profile, even at zero field, implying that there is a transverse fluctuation in velocity.

This fact is borne out in the experimental data shown in Fig. 5.10 which indicates that even for zero magnetic field (and its gradient) there is sizable broadening of the deflection profiles. This residual broadening, established from Eq. (5.67), is then added to all the theoretically computed line profile below, for a meaningful comparison with data. This discussion then also brings to fore the existence of two distinct temperatures in the problem: the oven temperature v already mentioned, which determines the jet-speed, and the lattice or the vibration temperature ¨ that governs the rotational relaxation of the magnetization of the cluster, as it tries to equilibrate to its own lattice through spinlattice relaxations. It is v that enters the discussion of the Fokker – Planck equation (5.25). (For a more detailed discussion on Ts and v see [117]). With the preceding background to the Stern-Gerlach geometry, the deflection d on the detector screen, measured from z = 0 (and upon ignoring ∆v¡ in Eq. (5.65)) can be written as ª«

ª«

3

3

P

¢© cos & ¢ cos . v 3

5.68

Clearly, d itself is a driven stochastic process, the mean value of which has to be computed from the expression (5.27), and the Kramers’

Memory in Nanomagnets

121

solution for the probability function P (θ , t ). that [118]

We have found earlier

R

¢© 1 ¢ 1 3 ¬ #GS 1 t®¯ª« ° & 1 t®¯ª« °'± ¢ z ©z z

1 © v 1 &¢ cos ¬ GSL & 1 #GS 1 t®¯ª« °'± . 2 v ©z z

5.69

where z is the Kramers’ relaxation rate that depends on the barrier height (anisotropy energy) and also the possible presence of a homogeneous component of the magnetic field in the Stern-Gerlach setup, < cos θ > eq is given by Eq. (5.4) and , is the initial polarization of the entering jet. Note that in the static limit z 0, applicable to the original Stern-Gerlach experiment, and for a fully polarized beam , 1, Eq. (5.69) reduces to Eq. (5.63), as we had anticipated earlier. The first step towards calculating the line profile, i.e., the intensity of ‘hits’ on the detector versus the deflection, requires the variance of the deflection. For computing the latter we want to evaluate the correlation function: < cos θ (0) cos θ (t ) >, which has been the subject of our earlier discussion (cf., Eq. (5.43)). But, now, cos is nonzero. We find 0cosθt

L 3 t®¯³ & ´3 1 t®¯³ °.

5.70

µµµL and from that, the variance The Eq. (5.70) is needed to compute L L µµµ R °, employing Eq. (5.69). While the variance is just the second comulant of the probability distribution of the deflection π ( d ) , in principle, all higher order cumulants are required to calculate the intensity profile. We find incredibly though that the second cumulant suffices i.e. the probability function π ( d ) is nearly a Gaussian [119]. The comparison with experimental data for Gd, and Co clusters is shown in Fig. 5.11 and Fig. 5.12 respectively. Figure 5.13 is a depiction of the intensity profile for Gd22 clusters which seems to point to a bidisperse

122

A Paradigm Called Magnetism

Fig. 5.11. Line profile for Gd23 and Gd22 clusters.

Fig. 5.12. Line profile for co-clusters, in zero and finite magnetic fields.

123

Memory in Nanomagnets

−4

−2

0 2 4 Deflection(mm)

6

8

Fig. 5.13. Double Gaussian profile for Gd22 indicating that there is a bi-modal size distribution.

distribution of sizes in the sample concerned. Thus we have a superposition of a set of clusters whose magnetization is frozen (τ > τ E ) and another set that exhibits superparamagnetism (τ < τ E ) . Mössbauer Relaxation of NiFe2O4 in SiO2 Matrix In this subsection we describe Mössbauer spectroscopy of single-domain nanomagnetic particles of NiFe2O4 embedded in a nonmagnetic SiO2 host. The samples are prepared by standard sol-gel techniques and are characterized by X-ray diffraction (XRD) and transmission electron microscopy (TEM) [120]. A rough description of three different kinds of samples used is shown in Fig. 5.14. The Table 1 below provides the relevant parameters:

124

A Paradigm Called Magnetism

Fig. 5.14. A schematic of sample sizes and their inter-particle separation.

Table 1 Sample Characteristics Average particle size Average inter-particle distance

Sample 1

Sample 2

Sample 3

3 nm

3 nm

15 nm

5 nm

15 nm

15 nm

In all cases the particle-size is found to follow a long-normal distribution which has the known attribute that dispersion goes hand in hand with the average size. Thus sample 3 with average particle size 15 nm is also expected to have the most pronounced dispersion compared to sample 1 and 2. We estimate that for sample 1, the interparticle dipolar interaction is the strongest because the average separation is about 5 nm. On the other hand, dipolar coupling is indeed very weak, for samples 2 and 3. Thus, sample 1 will be notionally referred to as “Interacting” while samples 2 and 3 as “Noninteracting”. This nomenclature is borne out by the room temperature hysteresis data, shown in Fig. 5.15. At room temperature the Neel relaxation is expected to be extremely rapid (cf. Eq. (5.11)) but the difference in the hysteresis curves for samples 2 and 3, in which sample 2 shows no hysteresis but sample 3 exhibits weak hysteresis, is precisely due to the size difference.

Memory in Nanomagnets

125

Fig. 5.15. Hysteresis behavior for samples 1, 2 and 3.

The 15 nm sized sample 3 has its relaxation time somewhat elongated (cf. Eq. (5.11)) compared to the 3 nm sized sample 2, and therefore, sample 3 requires a somewhat longer time to reach equilibrium. On the other hand, there is moderate hysteresis for sample 1 even though the average particle size 3 is the same as for sample 2; the reason is the dipolar interaction. For sample 1, the average interparticle separation is 5 nm and hence, the dipolar coupling, which is inversely proportional to the cube of inter-particle distance, is estimated to be stronger than in sample 2, again slowing down relaxation. In order to focus onto the effect of inter-particle interaction, keeping the average size fixed, we show temperature-dependent Mössbauer spectra in Fig. 5.16 for sample 1, and Fig. 5.17 for sample 2. The data at 20 K for both samples exhibit the characteristic six-finger pattern for 57Fe, contained in NiFe2O4, although sample 2 displays slight broadening of lines, implying that relaxation is not completely frozen, even at 20 K. As the temperature increases, relaxation speeds up and for sample 2 and at room temperature (RT), complete ‘motional narrowing’ sets in, yielding a single absorption line. Evidently, this speeding up of relaxation is not adequate for sample 1 which, even at RT, demonstrates

126

A Paradigm Called Magnetism

a split-lineshape. This effect is again attributed to the more pronounced dipolar interaction for sample 1 which competes with thermal energy in modulating the relaxation time scales. Thus, within the Mössbauer time window, which is nearly 10-8 sec corresponding to the lifetime of the excited nuclear state, the magnetization is apparently frozen for sample 1, even at room temperature! Relaxation Theory Within a Two State Model We have seen earlier that because of thermal fluctuations the magnetic moment undergoes rotational Brownian motion over an anisotropy barrier, in which the angle between the anisotropy axis and the magnetic moment vector is a continuous stochastic process. However the Kramers’ analysis showed that when KV>>kBT (in reality though KV can be a few times larger than kBT in order that the Kramers analysis is valid), the magnetic moment is mostly locked-in two orientations

0 and [, with slow relaxation between the two configurations. We are thus in the so called “Ising’ limit in which may be viewed as a dichotomic Markov process, in which it jumps at random between the angels 0 and [ at a rate given by the Arrhenius – Kramers formula (Eq. 5.10) (cf., also Fig. 4.1).

Fig. 5.16. Mössbauer lineshape for sample 1. Even RT spectre show split lines.

Memory in Nanomagnets

Fig. 5.17. Mössbauer spectre for sample 2. narrowing’.

127

The RT spectrum indicates ‘motional

We now discuss in somewhat more detail the effect of dipolar interaction. The latter is well known to yield complex magnetic order, being long-ranged, anisotropic and alternating in the sign of interaction. However, our hysteresis measurement, exhibited in Fig. 5.15, indicates that even for sample 1 for which the dipolar coupling is relevant, there is no shift of the hysteresis loop, thereby implying that the bulk magnetization, for the zero applied field, is zero. Our interpretation is that because of the largeness of the anisotropy barrier ¸ K we are in the Ising limit of the dipolar interaction, for which the local field, in the mean field sense, points parallel or antiparallel to the anisotropy axis, with equal probability. The dipolar interaction can now be described by its truncated form: ¹{t{

1 3 L º r Z Zº » ·¡ ·¡º , |¼º |½ º

L

5.71

where Z and Zº are the gyromagnetic ratio of the ith and jth particles respectively, WWWX ¼¾¿ is the vector distance between the sites at which the particles are located, º is the angle between the WWWX ¼¾¿ and the anisotropy axis and mzi is the (giant) magnetic moment for the ith nanoparticle along the anisotropy axis (i.e. Z). Given that m ¸ V, Eq. (71) may be rewritten as

128

A Paradigm Called Magnetism

¹{t{ L L r Z Zº »L º

1 3 L º º . ½ |¼WWWX ¾¿ |

5.72

Further, we assume the validity of mean field theory in which each nanomagnetic particle is imagined to be embedded in an effective medium that creates a local magnetic field at its site. The mean field (MF) form of Eq. (5.72) is ¥À ¹{t{ Z»L L r Zº » º

1 3 L º º , ½ |¼WWWX ¾¿ |

5.73

where the angular brackets < …. > represent a thermal average. Further, in accordance with our assumption about the largeness of the anisotropy energy, can be replaced by a two-state Ising variable Á: ¥À ¹{t{ Z»L L Á r Zº » º

1 3 L º Áº . ½ |¼WWWX ¾¿ |

5.74

In line with this approximation each particle can be viewed to be subjected to a local magnetic field H such that ¥À Á, ¹{t{

5.75

ÂÃ Á ,

5.76

ÂÃ ]" . k

5.77

where Â is a parameter that subsumes all the other constants. Within the proposed mean field theory, H can be expressed as (cf., Eq. (5.7))

Note that Eq. (5.77) admits both positive and negative solutions for H, in accordance with out discussion preceding Eq. (5.71). We now turn our attention to relaxation kinetics. Within the previously stated physical picture in which the Fokker-Planck process is replaced by a dichotomic Markov process we may write down the following set of rate equations for the number of magnetic particles with a specific orientations of their magnetization:

129

Memory in Nanomagnets

" Ä32 "3 &Ä23 "2 , 3 " Ä32 "3 Ä23 "2 , 2

5.78 5.79

where the subscripts on n indicate the two allowed values of . Solving Eqs. (5.78) and (5.79) we may derive for the time-dependent magnetization M(t): "3 "2

Å & 0 Ä

ΔÄ Å , 1 Ä Å Ä

where ", & "2 is normalized to unity, Å Ä32 &Ä23 , Ä

and

∆ Ä λ23 λ32 . GÇtM

GttM

5.80 5.81 5.82

Here Ä32 equals whereas Ä23 equals (cf., Eq. (5.11)). Furthermore, note that if M(t = 0) equals zero and ; K (linear response considered) Eq. (5.80) yields the earlier written expression in Eq. (5.12) wherein , is given by a combination of Eq. (5.3) and Eq. (5.7). Thus in the ‘high barrier – weak noise’ Kramers limit the two-state rate theory yields completely equivalent results as can be independently obtained from the Fokker-Planck description. Interpretation of the Mössbauer Spectra

The Mössbauer data shown in Fig. 5.16 and Fig. 5.17 are interpreted on the basis of the following stochastic model Hamiltonian: ¹ È ÉÊÊ¡ ,

5.83

where È is the nuclear magneton, g(I) is the level-specific g-factor ½ depending on whether the 57Fe nucleus is in its excited state I = L or the M L

ground state I = , Ê¡ is the component of the nuclear angular momentum

130

A Paradigm Called Magnetism

along the anisotropy direction, and h(t) is a local field at the nucleus that jumps about stochastically in time. The local field h(t) at the nucleus is of course produced by the magnetization of the particle which, for reasons outlined earlier, is taken to jump between Ë, , where , is proportional to H, given by Eq. (5.77). The rates at which these jumps occur are given by Ä32 and Ä23 . The Mössbauer lineshape as a function of the frequency is then given by [121, 122]. Ê

1 Ì r | Ê3 ·3 |Í |ÊM ·M |L [ ~ ~Î

tM

L L Ð È 3 É3 ·3 ÉM ·M L x Ï! & & Ñ Å Ä Ð 2 :! & 2< & 2

.

5.84

In Eq. (5.84) Í is the nuclear transition operator, the matrix elements of which are given by Clebsch-Gordan coefficients, Ð is the natural linewidth of the excited level, g’s are the ground and excited level g-factors Å is the volume-dependent rate given by Eq. (5.81). The and Ä integral over V incorporates the particle size distribution with the aid of a probability function f(V). As we mentioned earlier in connection with Fig. 5.15, the spectra are indicative of the presence of an apparently static magnetic field which is an internal field due to the dipolar interaction. The significant feature of the dipolar coupling is that the mean field H occurring in the exponent of the relaxation rates Ä32 and Ä23 is itself volume-dependent (cf., Eq. (5.77)). Therefore, the relaxation rates acquire an additional V2dependent term in the exponent, for the ‘Interacting’ sample 1. Thus, λ for a given temperature is systematically smaller for the interacting case (sample 1) than for the noninteracting case (sample 2). Hence, even at the room temperature the sample 1 displays a split spectrum, as discussed before. We may now summarize our interpretation of the observed Mössbauer spectra as follows. At any given point of time, half of Mössbauer nuclei find their ‘local’ magnetic field pointing along 0 while the other half will see the local field pointing along [. Both these orientations would of course yield an identical six-finger pattern, because the nucleus as an observer cannot distinguish between 0 and

Memory in Nanomagnets

131

[, provided the local field is static, within the Mössbauer measurement time. That of course is determined by the temperature T and the mean dipolar strength parametrized by Λ. These two quantities determine the rates of relaxation of the dipolar field. Hence, for sample 2, for which the dipolar field is negligible, semblance of a six-finger pattern shows up only at the lowest T when relaxation slows down, whereas for sample 1, the dipolar coupling keeps the relaxation slow within the nuclear time-window, at all temperatures. 5.4. Analysis of Results In the discussion of Mössbauer spectroscopy our focus has been the influence of dipolar interaction on slowing down relaxation. In this section we will turn our attention onto the effect of polydispersity, viz., volume-distribution of the nanoparticles. We will show that such a distribution leads to striking memory effects in low temperature DC magnetization measurements – surprisingly, and somewhat counter intuitively, dipolar interaction suppresses memory effects. The magnetization measurements are carried out in accordance with the following cooling and heating protocol (cf. Fig. 5.18). Starting from room temperature 300K , for our purpose), a small magnetic field of 100 Oe is applied and the magnetization (M) measured. Keeping the field on, the temperature (T) is lowered continuously at a steady rate of 20K/min and M is simultaneously measured upto the temperature Tn (the solid line). At Tn, the field is switched off and the drop of M is monitored for nearly 4 hours (dashed line). Subsequently, the field is switched back on and M(T) versus T is mapped in the cooling regime. Again at Tn-1 the field is switched off and the process of measurement is repeated, until the lowest temperature To is reached. Thus, one obtains field-cooled response and zero-field relaxation of the magnetization. At the end of the cooling cycle, at , , the field is turned on (dashed-dotted line), and M(T) is monitored as the system is heated from T0 through Tn-2, Tn-1, Tn and eventually to , again at the rate of 20K/min, the magnetic field remaining on, throughout. Our results are shown in Fig. 5.19, for samples 1, 2 and 3 (whose attributes are

132

A Paradigm Called Magnetism

Fig. 5.18. Time-temperature protocol.

Fig. 5.19. Magnetization versus temperature data during cooling and heating cycles, for samples 1, 2 and 3.

Memory in Nanomagnets

133

mentioned in Fig. 14 and Table 1). The heating path surprisingly shows wiggles in M(T) at all the T steps Tn-2, Tn-1, Tn where the magnetic field was earlier switched off during cooling, apparently retaining a memory of the temperature steps at which cooling was arrested. More surprising, however, is the fact that memory effects, defined here in terms of overlap of the data during cooling and heating cycles, are the most prominent for sample 3. Recall that for the latter dipolar interaction is negligible. Indeed memory effects are the weakest for the ‘Interacting’ sample 1. Our interpretation is that the observed memory effects are due to polydispersity, most prominent in sample 3, which leads to a superposition of relaxation times, because the volume V occurs in the exponent (cf. Eq. (5.10)). To illustrate this point, we now consider simulation data, for just two sizes (bidispersive), schematically depicted in Fig. 5.20. Recall that the ‘Blocking Temperature’ TB is that temperature at which the experimental timescale of measurement equals the relaxation time, i.e. τÓ τ3 exp :KVk T

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close